#------------------------------------------------------------------------------
#$Date: 2022-01-02 10:39:39 +0200 (Sun, 02 Jan 2022) $
#$Revision: 271679 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/30/50/4305049.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4305049
loop_
_publ_author_name
'Sheng-Qing Xia'
'Svilen Bobev'
_publ_contact_author_address
; 
Department of Chemistry and Biochemistry
304A Drake Hall
University of Delaware
Newark, DE 19716
USA
;
_publ_contact_author_email       sbobev@chem.udel.edu
_publ_contact_author_fax         'Intl. Code + (302) 8316335'
_publ_contact_author_phone       'Intl. Code + (302) 8318720'
_publ_section_title
;
Zintl Phase Variations Through Cation Selection. Synthesis and Structure of
A21Cd4Pn18 (A = Eu, Sr, Ba; Pn = Sb, Bi)
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1919
_journal_page_last               1921
_journal_paper_doi               10.1021/ic800242a
_journal_volume                  47
_journal_year                    2008
_chemical_formula_moiety         '2(Cd2 Sb6), 6(Sb), 21(Ba)'
_chemical_formula_sum            'Ba21 Cd4 Sb18'
_chemical_formula_weight         5525.24
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           64
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2ac 2'
_symmetry_space_group_name_H-M   'C m c e'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   18.191(6)
_cell_length_b                   19.103(6)
_cell_length_c                   37.062(11)
_cell_measurement_reflns_used    6813
_cell_measurement_temperature    120(2)
_cell_measurement_theta_max      26.37
_cell_measurement_theta_min      1.10
_cell_volume                     12879(7)
_computing_cell_refinement       'SMART (Bruker, 2000)'
_computing_data_collection       'SMART (Bruker, 2000)'
_computing_data_reduction        'SAINT (Bruker, 1999)'
_computing_molecular_graphics    'SHELXTL 5.1 (Sheldrick, 1994)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      120(2)
_diffrn_detector_area_resol_mean 8.3
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker Smart APEX'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0519
_diffrn_reflns_av_sigmaI/netI    0.0261
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       46
_diffrn_reflns_limit_l_min       -46
_diffrn_reflns_number            64901
_diffrn_reflns_theta_full        26.37
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         1.10
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    21.277
_exptl_absorpt_correction_T_max  0.345
_exptl_absorpt_correction_T_min  0.203
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 2003)'
_exptl_crystal_colour            Black
_exptl_crystal_density_diffrn    5.699
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Irregular
_exptl_crystal_F_000             18288
_exptl_crystal_size_max          0.11
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.05
_refine_diff_density_max         2.384
_refine_diff_density_min         -1.312
_refine_diff_density_rms         0.280
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.168
_refine_ls_matrix_type           full
_refine_ls_number_parameters     215
_refine_ls_number_reflns         6813
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.168
_refine_ls_R_factor_all          0.0291
_refine_ls_R_factor_gt           0.0245
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0145P)²+84.5894P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0484
_refine_ls_wR_factor_ref         0.0505
_reflns_number_gt                6223
_reflns_number_total             6813
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic800242a-file002_2.cif
_cod_data_source_block           Ba21Cd4Sb18
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Orthorhombic' changed to 'orthorhombic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

2022-01-02
Space group name changed to comply with IUCR recomendations
                 miguel
;
_cod_original_sg_symbol_H-M   'C m c a'
_cod_original_sg_symbol_Hall     '-C 2bc 2'
_cod_database_code               4305049
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y+1/2, z+1/2'
'-x, y+1/2, -z+1/2'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1, z+1/2'
'-x+1/2, y+1, -z+1/2'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y-1/2, -z-1/2'
'x, -y-1/2, z-1/2'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y, -z-1/2'
'x+1/2, -y, z-1/2'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ba1 Ba 0.12260(2) 0.39172(2) 0.277524(12) 0.01276(10) Uani 1 1 d . . .
Ba2 Ba 0.13164(2) 0.13895(2) 0.281358(12) 0.01273(10) Uani 1 1 d . . .
Ba3 Ba 0.15301(2) 0.08932(2) 0.075815(12) 0.01144(9) Uani 1 1 d . . .
Ba4 Ba 0.16072(2) 0.09703(2) 0.176866(11) 0.01117(9) Uani 1 1 d . . .
Ba5 Ba 0.17005(2) 0.43745(2) 0.170063(11) 0.01119(9) Uani 1 1 d . . .
Ba6 Ba 0.32462(2) 0.26413(2) 0.129030(11) 0.01093(9) Uani 1 1 d . . .
Ba7 Ba 0.33741(2) 0.16060(2) 0.031485(11) 0.01147(9) Uani 1 1 d . . .
Ba8 Ba 0.38034(2) 0.39230(2) 0.039138(12) 0.01214(9) Uani 1 1 d . . .
Ba9 Ba 0.0000 0.10429(4) 0.377737(17) 0.01416(14) Uani 1 2 d S . .
Ba10 Ba 0.0000 0.25553(3) 0.042351(17) 0.01218(13) Uani 1 2 d S . .
Ba11 Ba 0.0000 0.26888(3) 0.204129(16) 0.01153(13) Uani 1 2 d S . .
Ba12 Ba 0.12560(2) 0.44985(2) 0.060933(11) 0.01105(9) Uani 1 1 d . . .
Cd1 Cd 0.11776(3) 0.27035(3) 0.126884(14) 0.01143(11) Uani 1 1 d . . .
Cd2 Cd 0.0000 0.00978(4) 0.14552(2) 0.01400(16) Uani 1 2 d S . .
Cd3 Cd 0.0000 0.35163(4) 0.37311(2) 0.01174(16) Uani 1 2 d S . .
Sb1 Sb 0.19361(3) 0.27297(3) 0.057513(13) 0.01096(10) Uani 1 1 d . . .
Sb2 Sb 0.19660(3) 0.26790(3) 0.200732(13) 0.01093(10) Uani 1 1 d . . .
Sb3 Sb 0.31774(3) 0.08797(3) 0.121782(13) 0.01063(10) Uani 1 1 d . . .
Sb4 Sb 0.36409(3) 0.43889(3) 0.130172(12) 0.01016(10) Uani 1 1 d . . .
Sb5 Sb 0.0000 0.04531(4) 0.030094(18) 0.01206(15) Uani 1 2 d S . .
Sb6 Sb 0.0000 0.06041(4) 0.222837(18) 0.01124(14) Uani 1 2 d S . .
Sb7 Sb 0.0000 0.06939(4) 0.484151(18) 0.01098(14) Uani 1 2 d S . .
Sb8 Sb 0.0000 0.15911(4) 0.125255(18) 0.00989(14) Uani 1 2 d S . .
Sb9 Sb 0.0000 0.25532(4) 0.436280(18) 0.01086(14) Uani 1 2 d S . .
Sb10 Sb 0.0000 0.25767(4) 0.310709(18) 0.01039(14) Uani 1 2 d S . .
Sb11 Sb 0.0000 0.37902(4) 0.123614(18) 0.01038(14) Uani 1 2 d S . .
Sb12 Sb 0.0000 0.47807(4) 0.211815(18) 0.01213(15) Uani 1 2 d S . .
Sb13 Sb 0.2500 0.01327(4) 0.2500 0.00927(14) Uani 1 2 d S . .
Sb14 Sb 0.24567(4) 0.0000 0.0000 0.01014(14) Uani 1 2 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cd Cd -0.8075 1.2024 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Sb13 Ba1 Sb4 93.934(18) 10_566 7_545 ?
Sb13 Ba1 Sb10 175.467(17) 10_566 . ?
Sb4 Ba1 Sb10 83.91(2) 7_545 . ?
Sb13 Ba1 Sb12 84.81(2) 10_566 . ?
Sb4 Ba1 Sb12 124.34(2) 7_545 . ?
Sb10 Ba1 Sb12 99.70(2) . . ?
Sb13 Ba1 Sb6 80.04(3) 10_566 10_566 ?
Sb4 Ba1 Sb6 80.396(16) 7_545 10_566 ?
Sb10 Ba1 Sb6 103.46(3) . 10_566 ?
Sb12 Ba1 Sb6 44.476(18) . 10_566 ?
Sb13 Ba1 Sb2 87.75(2) 10_566 . ?
Sb4 Ba1 Sb2 145.750(19) 7_545 . ?
Sb10 Ba1 Sb2 91.80(3) . . ?
Sb12 Ba1 Sb2 89.89(3) . . ?
Sb6 Ba1 Sb2 133.31(2) 10_566 . ?
Sb13 Ba1 Ba5 55.589(9) 10_566 . ?
Sb4 Ba1 Ba5 148.70(2) 7_545 . ?
Sb10 Ba1 Ba5 127.009(17) . . ?
Sb12 Ba1 Ba5 53.201(18) . . ?
Sb6 Ba1 Ba5 86.686(16) 10_566 . ?
Sb2 Ba1 Ba5 50.541(19) . . ?
Sb13 Ba1 Ba11 122.67(2) 10_566 . ?
Sb4 Ba1 Ba11 142.910(18) 7_545 . ?
Sb10 Ba1 Ba11 59.99(2) . . ?
Sb12 Ba1 Ba11 60.33(2) . . ?
Sb6 Ba1 Ba11 98.86(2) 10_566 . ?
Sb2 Ba1 Ba11 51.831(19) . . ?
Ba5 Ba1 Ba11 67.10(2) . . ?
Sb13 Ba1 Ba4 52.786(17) 10_566 10_566 ?
Sb4 Ba1 Ba4 51.814(12) 7_545 10_566 ?
Sb10 Ba1 Ba4 127.49(2) . 10_566 ?
Sb12 Ba1 Ba4 87.10(2) . 10_566 ?
Sb6 Ba1 Ba4 49.243(19) 10_566 10_566 ?
Sb2 Ba1 Ba4 140.536(17) . 10_566 ?
Ba5 Ba1 Ba4 98.631(19) . 10_566 ?
Ba11 Ba1 Ba4 147.023(15) . 10_566 ?
Sb13 Ba1 Ba5 53.804(16) 10_566 7_545 ?
Sb4 Ba1 Ba5 57.088(14) 7_545 7_545 ?
Sb10 Ba1 Ba5 121.87(2) . 7_545 ?
Sb12 Ba1 Ba5 137.038(19) . 7_545 ?
Sb6 Ba1 Ba5 109.34(2) 10_566 7_545 ?
Sb2 Ba1 Ba5 98.49(2) . 7_545 ?
Ba5 Ba1 Ba5 101.883(19) . 7_545 ?
Ba11 Ba1 Ba5 149.281(15) . 7_545 ?
Ba4 Ba1 Ba5 60.161(11) 10_566 7_545 ?
Sb13 Ba1 Ba6 117.839(19) 10_566 7_545 ?
Sb4 Ba1 Ba6 50.07(2) 7_545 7_545 ?
Sb10 Ba1 Ba6 57.792(18) . 7_545 ?
Sb12 Ba1 Ba6 155.588(16) . 7_545 ?
Sb6 Ba1 Ba6 126.162(19) 10_566 7_545 ?
Sb2 Ba1 Ba6 99.42(3) . 7_545 ?
Ba5 Ba1 Ba6 146.513(18) . 7_545 ?
Ba11 Ba1 Ba6 108.56(2) . 7_545 ?
Ba4 Ba1 Ba6 99.31(2) 10_566 7_545 ?
Ba5 Ba1 Ba6 64.087(15) 7_545 7_545 ?
Sb13 Ba1 Ba1 132.419(15) 10_566 12 ?
Sb4 Ba1 Ba1 93.915(11) 7_545 12 ?
Sb10 Ba1 Ba1 51.867(15) . 12 ?
Sb12 Ba1 Ba1 52.830(14) . 12 ?
Sb6 Ba1 Ba1 55.315(15) 10_566 12 ?
Sb2 Ba1 Ba1 109.989(12) . 12 ?
Ba5 Ba1 Ba1 101.952(10) . 12 ?
Ba11 Ba1 Ba1 58.168(12) . 12 ?
Ba4 Ba1 Ba1 99.222(9) 10_566 12 ?
Ba5 Ba1 Ba1 150.547(13) 7_545 12 ?
Ba6 Ba1 Ba1 102.776(9) 7_545 12 ?
Sb13 Ba2 Sb10 175.316(18) . . ?
Sb13 Ba2 Sb6 85.46(2) . . ?
Sb10 Ba2 Sb6 90.13(2) . . ?
Sb13 Ba2 Sb3 89.350(19) . 7_545 ?
Sb10 Ba2 Sb3 92.19(2) . 7_545 ?
Sb6 Ba2 Sb3 128.67(2) . 7_545 ?
Sb13 Ba2 Sb12 81.72(3) . 10_556 ?
Sb10 Ba2 Sb12 94.06(3) . 10_556 ?
Sb6 Ba2 Sb12 45.222(19) . 10_556 ?
Sb3 Ba2 Sb12 83.487(17) 7_545 10_556 ?
Sb13 Ba2 Ba4 56.431(10) . . ?
Sb10 Ba2 Ba4 121.771(17) . . ?
Sb6 Ba2 Ba4 54.099(18) . . ?
Sb3 Ba2 Ba4 145.73(2) 7_545 . ?
Sb12 Ba2 Ba4 89.213(16) 10_556 . ?
Sb13 Ba2 Sb2 89.83(3) . 7_545 ?
Sb10 Ba2 Sb2 94.81(3) . 7_545 ?
Sb6 Ba2 Sb2 151.414(19) . 7_545 ?
Sb3 Ba2 Sb2 79.334(16) 7_545 7_545 ?
Sb12 Ba2 Sb2 160.929(17) 10_556 7_545 ?
Ba4 Ba2 Sb2 100.346(15) . 7_545 ?
Sb13 Ba2 Sb2 89.58(2) . . ?
Sb10 Ba2 Sb2 92.01(2) . . ?
Sb6 Ba2 Sb2 90.18(3) . . ?
Sb3 Ba2 Sb2 140.888(19) 7_545 . ?
Sb12 Ba2 Sb2 134.891(19) 10_556 . ?
Ba4 Ba2 Sb2 50.733(19) . . ?
Sb2 Ba2 Sb2 61.57(2) 7_545 . ?
Sb13 Ba2 Ba4 54.623(16) . 7_545 ?
Sb10 Ba2 Ba4 129.44(2) . 7_545 ?
Sb6 Ba2 Ba4 139.10(2) . 7_545 ?
Sb3 Ba2 Ba4 51.992(11) 7_545 7_545 ?
Sb12 Ba2 Ba4 112.41(2) 10_556 7_545 ?
Ba4 Ba2 Ba4 101.666(17) . 7_545 ?
Sb2 Ba2 Ba4 49.68(2) 7_545 7_545 ?
Sb2 Ba2 Ba4 97.28(2) . 7_545 ?
Sb13 Ba2 Ba6 123.499(19) . 7_545 ?
Sb10 Ba2 Ba6 60.497(19) . 7_545 ?
Sb6 Ba2 Ba6 148.749(17) . 7_545 ?
Sb3 Ba2 Ba6 49.73(2) 7_545 7_545 ?
Sb12 Ba2 Ba6 121.13(2) 10_556 7_545 ?
Ba4 Ba2 Ba6 149.659(17) . 7_545 ?
Sb2 Ba2 Ba6 51.010(13) 7_545 7_545 ?
Sb2 Ba2 Ba6 100.56(3) . 7_545 ?
Ba4 Ba2 Ba6 68.939(14) 7_545 7_545 ?
Sb13 Ba2 Ba5 54.114(18) . 10_556 ?
Sb10 Ba2 Ba5 124.37(2) . 10_556 ?
Sb6 Ba2 Ba5 89.26(2) . 10_556 ?
Sb3 Ba2 Ba5 48.865(11) 7_545 10_556 ?
Sb12 Ba2 Ba5 50.864(19) 10_556 10_556 ?
Ba4 Ba2 Ba5 101.823(19) . 10_556 ?
Sb2 Ba2 Ba5 110.57(2) 7_545 10_556 ?
Sb2 Ba2 Ba5 143.609(16) . 10_556 ?
Ba4 Ba2 Ba5 61.643(11) 7_545 10_556 ?
Ba6 Ba2 Ba5 98.55(2) 7_545 10_556 ?
Sb13 Ba2 Ba9 121.16(2) . . ?
Sb10 Ba2 Ba9 57.505(19) . . ?
Sb6 Ba2 Ba9 93.77(3) . . ?
Sb3 Ba2 Ba9 47.505(19) 7_545 . ?
Sb12 Ba2 Ba9 59.298(17) 10_556 . ?
Ba4 Ba2 Ba9 147.062(18) . . ?
Sb2 Ba2 Ba9 112.59(2) 7_545 . ?
Sb2 Ba2 Ba9 149.215(18) . . ?
Ba4 Ba2 Ba9 99.49(2) 7_545 . ?
Ba6 Ba2 Ba9 62.51(2) 7_545 . ?
Ba5 Ba2 Ba9 67.048(15) 10_556 . ?
Sb5 Ba3 Sb3 165.01(2) . . ?
Sb5 Ba3 Sb4 90.64(2) . 16_545 ?
Sb3 Ba3 Sb4 77.763(18) . 16_545 ?
Sb5 Ba3 Sb8 73.05(3) . . ?
Sb3 Ba3 Sb8 115.13(3) . . ?
Sb4 Ba3 Sb8 86.71(2) 16_545 . ?
Sb5 Ba3 Sb1 108.30(2) . . ?
Sb3 Ba3 Sb1 85.591(16) . . ?
Sb4 Ba3 Sb1 155.284(19) 16_545 . ?
Sb8 Ba3 Sb1 83.96(2) . . ?
Sb5 Ba3 Sb14 83.05(3) . . ?
Sb3 Ba3 Sb14 88.61(2) . . ?
Sb4 Ba3 Sb14 95.65(2) 16_545 . ?
Sb8 Ba3 Sb14 156.020(18) . . ?
Sb1 Ba3 Sb14 102.14(2) . . ?
Sb5 Ba3 Ba4 122.924(19) . . ?
Sb3 Ba3 Ba4 58.285(16) . . ?
Sb4 Ba3 Ba4 57.613(17) 16_545 . ?
Sb8 Ba3 Ba4 60.308(17) . . ?
Sb1 Ba3 Ba4 98.066(15) . . ?
Sb14 Ba3 Ba4 139.511(19) . . ?
Sb5 Ba3 Ba7 125.12(3) . . ?
Sb3 Ba3 Ba7 58.22(2) . . ?
Sb4 Ba3 Ba7 126.166(17) 16_545 . ?
Sb8 Ba3 Ba7 137.57(2) . . ?
Sb1 Ba3 Ba7 54.768(12) . . ?
Sb14 Ba3 Ba7 57.240(17) . . ?
Ba4 Ba3 Ba7 111.570(17) . . ?
Sb5 Ba3 Cd1 108.79(2) . . ?
Sb3 Ba3 Cd1 84.943(17) . . ?
Sb4 Ba3 Cd1 114.90(3) 16_545 . ?
Sb8 Ba3 Cd1 46.526(15) . . ?
Sb1 Ba3 Cd1 44.61(2) . . ?
Sb14 Ba3 Cd1 146.468(15) . . ?
Ba4 Ba3 Cd1 59.922(15) . . ?
Ba7 Ba3 Cd1 91.992(19) . . ?
Sb5 Ba3 Ba8 58.305(16) . 16_545 ?
Sb3 Ba3 Ba8 106.816(17) . 16_545 ?
Sb4 Ba3 Ba8 54.57(2) 16_545 16_545 ?
Sb8 Ba3 Ba8 113.619(19) . 16_545 ?
Sb1 Ba3 Ba8 149.54(2) . 16_545 ?
Sb14 Ba3 Ba8 51.933(13) . 16_545 ?
Ba4 Ba3 Ba8 112.179(16) . 16_545 ?
Ba7 Ba3 Ba8 107.825(16) . 16_545 ?
Cd1 Ba3 Ba8 160.094(17) . 16_545 ?
Sb5 Ba3 Cd2 70.27(3) . . ?
Sb3 Ba3 Cd2 106.06(3) . . ?
Sb4 Ba3 Cd2 43.595(15) 16_545 . ?
Sb8 Ba3 Cd2 44.59(2) . . ?
Sb1 Ba3 Cd2 127.760(18) . . ?
Sb14 Ba3 Cd2 128.26(2) . . ?
Ba4 Ba3 Cd2 53.800(18) . . ?
Ba7 Ba3 Cd2 164.242(16) . . ?
Cd1 Ba3 Cd2 85.02(2) . . ?
Ba8 Ba3 Cd2 76.39(2) 16_545 . ?
Sb5 Ba3 Ba8 53.649(15) . 13 ?
Sb3 Ba3 Ba8 127.617(17) . 13 ?
Sb4 Ba3 Ba8 128.179(18) 16_545 13 ?
Sb8 Ba3 Ba8 111.38(2) . 13 ?
Sb1 Ba3 Ba8 76.516(13) . 13 ?
Sb14 Ba3 Ba8 49.545(17) . 13 ?
Ba4 Ba3 Ba8 170.877(16) . 13 ?
Ba7 Ba3 Ba8 71.514(16) . 13 ?
Cd1 Ba3 Ba8 112.003(18) . 13 ?
Ba8 Ba3 Ba8 73.926(16) 16_545 13 ?
Cd2 Ba3 Ba8 123.90(2) . 13 ?
Sb2 Ba4 Sb6 103.04(2) . . ?
Sb2 Ba4 Sb4 165.122(19) . 16_545 ?
Sb6 Ba4 Sb4 87.71(2) . 16_545 ?
Sb2 Ba4 Sb3 92.399(17) . . ?
Sb6 Ba4 Sb3 164.56(2) . . ?
Sb4 Ba4 Sb3 77.046(18) 16_545 . ?
Sb2 Ba4 Sb13 98.32(2) . . ?
Sb6 Ba4 Sb13 85.36(2) . . ?
Sb4 Ba4 Sb13 92.72(2) 16_545 . ?
Sb3 Ba4 Sb13 92.84(2) . . ?
Sb2 Ba4 Cd2 133.085(19) . . ?
Sb6 Ba4 Cd2 51.05(2) . . ?
Sb4 Ba4 Cd2 47.987(16) 16_545 . ?
Sb3 Ba4 Cd2 117.05(3) . . ?
Sb13 Ba4 Cd2 114.51(2) . . ?
Sb2 Ba4 Sb8 88.78(2) . . ?
Sb6 Ba4 Sb8 69.53(3) . . ?
Sb4 Ba4 Sb8 85.36(2) 16_545 . ?
Sb3 Ba4 Sb8 111.02(3) . . ?
Sb13 Ba4 Sb8 154.865(16) . . ?
Cd2 Ba4 Sb8 47.98(2) . . ?
Sb2 Ba4 Ba3 107.502(16) . . ?
Sb6 Ba4 Ba3 116.92(2) . . ?
Sb4 Ba4 Ba3 57.941(16) 16_545 . ?
Sb3 Ba4 Ba3 56.534(18) . . ?
Sb13 Ba4 Ba3 139.779(19) . . ?
Cd2 Ba4 Ba3 67.978(17) . . ?
Sb8 Ba4 Ba3 57.677(16) . . ?
Sb2 Ba4 Cd1 49.53(2) . . ?
Sb6 Ba4 Cd1 103.78(2) . . ?
Sb4 Ba4 Cd1 118.29(3) 16_545 . ?
Sb3 Ba4 Cd1 85.889(18) . . ?
Sb13 Ba4 Cd1 147.632(18) . . ?
Cd2 Ba4 Cd1 94.50(2) . . ?
Sb8 Ba4 Cd1 46.959(15) . . ?
Ba3 Ba4 Cd1 63.160(17) . . ?
Sb2 Ba4 Ba2 65.521(13) . . ?
Sb6 Ba4 Ba2 56.623(16) . . ?
Sb4 Ba4 Ba2 129.354(17) 16_545 . ?
Sb3 Ba4 Ba2 132.948(18) . . ?
Sb13 Ba4 Ba2 53.749(19) . . ?
Cd2 Ba4 Ba2 107.57(2) . . ?
Sb8 Ba4 Ba2 109.49(2) . . ?
Ba3 Ba4 Ba2 166.441(17) . . ?
Cd1 Ba4 Ba2 105.42(2) . . ?
Sb2 Ba4 Ba2 63.253(13) . 7_545 ?
Sb6 Ba4 Ba2 128.59(2) . 7_545 ?
Sb4 Ba4 Ba2 117.765(16) 16_545 7_545 ?
Sb3 Ba4 Ba2 59.19(2) . 7_545 ?
Sb13 Ba4 Ba2 52.104(14) . 7_545 ?
Cd2 Ba4 Ba2 163.173(19) . 7_545 ?
Sb8 Ba4 Ba2 148.28(2) . 7_545 ?
Ba3 Ba4 Ba2 114.405(16) . 7_545 ?
Cd1 Ba4 Ba2 101.341(18) . 7_545 ?
Ba2 Ba4 Ba2 73.768(17) . 7_545 ?
Sb2 Ba4 Ba1 142.10(2) . 10_556 ?
Sb6 Ba4 Ba1 59.219(15) . 10_556 ?
Sb4 Ba4 Ba1 52.55(2) 16_545 10_556 ?
Sb3 Ba4 Ba1 108.210(17) . 10_556 ?
Sb13 Ba4 Ba1 50.581(15) . 10_556 ?
Cd2 Ba4 Ba1 64.628(19) . 10_556 ?
Sb8 Ba4 Ba1 111.524(19) . 10_556 ?
Ba3 Ba4 Ba1 110.397(17) . 10_556 ?
Cd1 Ba4 Ba1 158.326(18) . 10_556 ?
Ba2 Ba4 Ba1 77.377(18) . 10_556 ?
Ba2 Ba4 Ba1 100.055(14) 7_545 10_556 ?
Sb3 Ba5 Sb2 162.818(19) 16 . ?
Sb3 Ba5 Sb12 95.84(2) 16 . ?
Sb2 Ba5 Sb12 100.54(2) . . ?
Sb3 Ba5 Sb13 93.81(2) 16 10_566 ?
Sb2 Ba5 Sb13 92.85(2) . 10_566 ?
Sb12 Ba5 Sb13 84.57(2) . 10_566 ?
Sb3 Ba5 Cd1 121.36(3) 16 . ?
Sb2 Ba5 Cd1 51.00(2) . . ?
Sb12 Ba5 Cd1 98.83(2) . . ?
Sb13 Ba5 Cd1 143.801(18) 10_566 . ?
Sb3 Ba5 Sb11 93.72(2) 16 . ?
Sb2 Ba5 Sb11 89.27(2) . . ?
Sb12 Ba5 Sb11 62.68(2) . . ?
Sb13 Ba5 Sb11 146.967(16) 10_566 . ?
Cd1 Ba5 Sb11 47.537(15) . . ?
Sb3 Ba5 Sb4 74.329(15) 16 . ?
Sb2 Ba5 Sb4 90.279(16) . . ?
Sb12 Ba5 Sb4 166.40(2) . . ?
Sb13 Ba5 Sb4 86.70(2) 10_566 . ?
Cd1 Ba5 Sb4 94.377(18) . . ?
Sb11 Ba5 Sb4 126.27(2) . . ?
Sb3 Ba5 Ba12 56.502(15) 16 . ?
Sb2 Ba5 Ba12 113.694(16) . . ?
Sb12 Ba5 Ba12 104.12(2) . . ?
Sb13 Ba5 Ba12 149.391(19) 10_566 . ?
Cd1 Ba5 Ba12 64.861(16) . . ?
Sb11 Ba5 Ba12 53.138(14) . . ?
Sb4 Ba5 Ba12 78.576(18) . . ?
Sb3 Ba5 Ba1 134.026(17) 16 . ?
Sb2 Ba5 Ba1 61.290(13) . . ?
Sb12 Ba5 Ba1 56.496(15) . . ?
Sb13 Ba5 Ba1 51.85(2) 10_566 . ?
Cd1 Ba5 Ba1 100.34(2) . . ?
Sb11 Ba5 Ba1 101.98(2) . . ?
Sb4 Ba5 Ba1 124.171(15) . . ?
Ba12 Ba5 Ba1 155.093(18) . . ?
Sb3 Ba5 Ba2 58.25(2) 16 10_566 ?
Sb2 Ba5 Ba2 136.11(2) . 10_566 ?
Sb12 Ba5 Ba2 58.685(15) . 10_566 ?
Sb13 Ba5 Ba2 50.404(14) 10_566 10_566 ?
Cd1 Ba5 Ba2 155.698(19) . 10_566 ?
Sb11 Ba5 Ba2 109.116(19) . 10_566 ?
Sb4 Ba5 Ba2 107.743(15) . 10_566 ?
Ba12 Ba5 Ba2 109.046(17) . 10_566 ?
Ba1 Ba5 Ba2 75.773(18) . 10_566 ?
Sb3 Ba5 Ba1 110.506(18) 16 7_545 ?
Sb2 Ba5 Ba1 62.818(13) . 7_545 ?
Sb12 Ba5 Ba1 127.46(3) . 7_545 ?
Sb13 Ba5 Ba1 50.286(13) 10_566 7_545 ?
Cd1 Ba5 Ba1 104.129(19) . 7_545 ?
Sb11 Ba5 Ba1 150.81(2) . 7_545 ?
Sb4 Ba5 Ba1 51.06(2) . 7_545 ?
Ba12 Ba5 Ba1 128.389(14) . 7_545 ?
Ba1 Ba5 Ba1 73.114(19) . 7_545 ?
Ba2 Ba5 Ba1 97.704(15) 10_566 7_545 ?
Sb3 Ba5 Ba4 52.346(17) 16 16 ?
Sb2 Ba5 Ba4 122.58(2) . 16 ?
Sb12 Ba5 Ba4 116.10(2) . 16 ?
Sb13 Ba5 Ba4 51.953(13) 10_566 16 ?
Cd1 Ba5 Ba4 144.542(18) . 16 ?
Sb11 Ba5 Ba4 146.032(19) . 16 ?
Sb4 Ba5 Ba4 50.441(17) . 16 ?
Ba12 Ba5 Ba4 98.944(13) . 16 ?
Ba1 Ba5 Ba4 103.806(15) . 16 ?
Ba2 Ba5 Ba4 57.517(19) 10_566 16 ?
Ba1 Ba5 Ba4 59.86(2) 7_545 16 ?
Sb3 Ba6 Sb4 169.284(19) . . ?
Sb3 Ba6 Sb2 93.192(16) . . ?
Sb4 Ba6 Sb2 96.277(16) . . ?
Sb3 Ba6 Sb1 87.898(15) . . ?
Sb4 Ba6 Sb1 95.937(16) . . ?
Sb2 Ba6 Sb1 96.75(3) . . ?
Sb3 Ba6 Cd3 119.55(2) . 14_556 ?
Sb4 Ba6 Cd3 50.244(16) . 14_556 ?
Sb2 Ba6 Cd3 126.20(2) . 14_556 ?
Sb1 Ba6 Cd3 123.59(2) . 14_556 ?
Sb3 Ba6 Cd1 89.586(16) . . ?
Sb4 Ba6 Cd1 100.344(17) . . ?
Sb2 Ba6 Cd1 49.967(18) . . ?
Sb1 Ba6 Cd1 46.799(17) . . ?
Cd3 Ba6 Cd1 150.44(2) 14_556 . ?
Sb3 Ba6 Sb10 92.539(17) . 14_556 ?
Sb4 Ba6 Sb10 81.472(17) . 14_556 ?
Sb2 Ba6 Sb10 96.27(3) . 14_556 ?
Sb1 Ba6 Sb10 166.934(17) . 14_556 ?
Cd3 Ba6 Sb10 45.75(2) 14_556 14_556 ?
Cd1 Ba6 Sb10 146.23(2) . 14_556 ?
Sb3 Ba6 Sb9 86.535(16) . 14_556 ?
Sb4 Ba6 Sb9 83.177(17) . 14_556 ?
Sb2 Ba6 Sb9 168.355(17) . 14_556 ?
Sb1 Ba6 Sb9 94.88(3) . 14_556 ?
Cd3 Ba6 Sb9 45.68(2) 14_556 14_556 ?
Cd1 Ba6 Sb9 141.63(2) . 14_556 ?
Sb10 Ba6 Sb9 72.13(3) 14_556 14_556 ?
Sb3 Ba6 Ba7 56.981(15) . . ?
Sb4 Ba6 Ba7 117.869(18) . . ?
Sb2 Ba6 Ba7 134.87(2) . . ?
Sb1 Ba6 Ba7 53.824(19) . . ?
Cd3 Ba6 Ba7 98.809(18) 14_556 . ?
Cd1 Ba6 Ba7 93.037(14) . . ?
Sb10 Ba6 Ba7 116.15(2) 14_556 . ?
Sb9 Ba6 Ba7 53.561(16) 14_556 . ?
Sb3 Ba6 Ba2 59.937(18) . 7_545 ?
Sb4 Ba6 Ba2 120.710(19) . 7_545 ?
Sb2 Ba6 Ba2 62.51(2) . 7_545 ?
Sb1 Ba6 Ba2 138.271(19) . 7_545 ?
Cd3 Ba6 Ba2 96.58(2) 14_556 7_545 ?
Cd1 Ba6 Ba2 103.042(15) . 7_545 ?
Sb10 Ba6 Ba2 50.869(15) 14_556 7_545 ?
Sb9 Ba6 Ba2 107.76(2) 14_556 7_545 ?
Ba7 Ba6 Ba2 114.34(3) . 7_545 ?
Sb3 Ba6 Ba8 121.30(2) . . ?
Sb4 Ba6 Ba8 52.943(16) . . ?
Sb2 Ba6 Ba8 137.194(19) . . ?
Sb1 Ba6 Ba8 63.29(2) . . ?
Cd3 Ba6 Ba8 60.336(16) 14_556 . ?
Cd1 Ba6 Ba8 101.728(15) . . ?
Sb10 Ba6 Ba8 105.78(2) 14_556 . ?
Sb9 Ba6 Ba8 50.360(16) 14_556 . ?
Ba7 Ba6 Ba8 64.96(2) . . ?
Ba2 Ba6 Ba8 155.215(18) 7_545 . ?
Sb3 Ba6 Ba1 129.102(18) . 7_545 ?
Sb4 Ba6 Ba1 52.767(16) . 7_545 ?
Sb2 Ba6 Ba1 62.26(2) . 7_545 ?
Sb1 Ba6 Ba1 135.525(19) . 7_545 ?
Cd3 Ba6 Ba1 63.977(17) 14_556 7_545 ?
Cd1 Ba6 Ba1 102.716(15) . 7_545 ?
Sb10 Ba6 Ba1 51.652(15) 14_556 7_545 ?
Sb9 Ba6 Ba1 109.22(2) 14_556 7_545 ?
Ba7 Ba6 Ba1 162.756(16) . 7_545 ?
Ba2 Ba6 Ba1 69.17(3) 7_545 7_545 ?
Ba8 Ba6 Ba1 104.40(3) . 7_545 ?
Sb7 Ba7 Sb1 169.284(19) 14_556 . ?
Sb7 Ba7 Sb1 99.09(2) 14_556 13 ?
Sb1 Ba7 Sb1 85.36(2) . 13 ?
Sb7 Ba7 Sb3 92.623(19) 14_556 . ?
Sb1 Ba7 Sb3 84.687(19) . . ?
Sb1 Ba7 Sb3 165.214(18) 13 . ?
Sb7 Ba7 Sb9 67.42(3) 14_556 14_556 ?
Sb1 Ba7 Sb9 102.08(3) . 14_556 ?
Sb1 Ba7 Sb9 104.62(2) 13 14_556 ?
Sb3 Ba7 Sb9 88.16(2) . 14_556 ?
Sb7 Ba7 Sb14 85.14(3) 14_556 . ?
Sb1 Ba7 Sb14 104.96(3) . . ?
Sb1 Ba7 Sb14 86.096(19) 13 . ?
Sb3 Ba7 Sb14 85.94(2) . . ?
Sb9 Ba7 Sb14 151.624(18) 14_556 . ?
Sb7 Ba7 Ba3 127.90(3) 14_556 . ?
Sb1 Ba7 Ba3 57.88(2) . . ?
Sb1 Ba7 Ba3 111.67(2) 13 . ?
Sb3 Ba7 Ba3 53.605(13) . . ?
Sb9 Ba7 Ba3 135.63(2) 14_556 . ?
Sb14 Ba7 Ba3 57.535(16) . . ?
Sb7 Ba7 Ba12 57.397(15) 14_556 13 ?
Sb1 Ba7 Ba12 131.946(17) . 13 ?
Sb1 Ba7 Ba12 55.63(2) 13 13 ?
Sb3 Ba7 Ba12 126.23(2) . 13 ?
Sb9 Ba7 Ba12 113.31(2) 14_556 13 ?
Sb14 Ba7 Ba12 51.513(14) . 13 ?
Ba3 Ba7 Ba12 108.003(18) . 13 ?
Sb7 Ba7 Ba6 115.691(18) 14_556 . ?
Sb1 Ba7 Ba6 54.944(14) . . ?
Sb1 Ba7 Ba6 128.93(2) 13 . ?
Sb3 Ba7 Ba6 51.09(2) . . ?
Sb9 Ba7 Ba6 61.556(17) 14_556 . ?
Sb14 Ba7 Ba6 130.637(15) . . ?
Ba3 Ba7 Ba6 75.792(17) . . ?
Ba12 Ba7 Ba6 173.086(15) 13 . ?
Sb7 Ba7 Ba12 55.306(15) 14_556 16_545 ?
Sb1 Ba7 Ba12 128.966(18) . 16_545 ?
Sb1 Ba7 Ba12 126.945(15) 13 16_545 ?
Sb3 Ba7 Ba12 54.202(12) . 16_545 ?
Sb9 Ba7 Ba12 104.92(2) 14_556 16_545 ?
Sb14 Ba7 Ba12 50.220(18) . 16_545 ?
Ba3 Ba7 Ba12 72.621(16) . 16_545 ?
Ba12 Ba7 Ba12 72.41(2) 13 16_545 ?
Ba6 Ba7 Ba12 103.85(2) . 16_545 ?
Sb7 Ba7 Ba10 60.03(2) 14_556 13 ?
Sb1 Ba7 Ba10 117.04(2) . 13 ?
Sb1 Ba7 Ba10 52.764(19) 13 13 ?
Sb3 Ba7 Ba10 142.000(18) . 13 ?
Sb9 Ba7 Ba10 58.21(2) 14_556 13 ?
Sb14 Ba7 Ba10 114.64(2) . 13 ?
Ba3 Ba7 Ba10 164.331(15) . 13 ?
Ba12 Ba7 Ba10 63.17(2) 13 13 ?
Ba6 Ba7 Ba10 114.47(2) . 13 ?
Ba12 Ba7 Ba10 113.983(17) 16_545 13 ?
Sb7 Ba7 Ba8 110.80(2) 14_556 . ?
Sb1 Ba7 Ba8 60.795(19) . . ?
Sb1 Ba7 Ba8 74.743(16) 13 . ?
Sb3 Ba7 Ba8 109.494(17) . . ?
Sb9 Ba7 Ba8 49.814(14) 14_556 . ?
Sb14 Ba7 Ba8 156.549(16) . . ?
Ba3 Ba7 Ba8 117.184(14) . . ?
Ba12 Ba7 Ba8 122.188(16) 13 . ?
Ba6 Ba7 Ba8 58.911(13) . . ?
Ba12 Ba7 Ba8 153.204(17) 16_545 . ?
Ba10 Ba7 Ba8 63.790(14) 13 . ?
Sb14 Ba8 Sb4 101.54(2) 13 . ?
Sb14 Ba8 Sb9 167.127(18) 13 14_556 ?
Sb4 Ba8 Sb9 89.53(2) . 14_556 ?
Sb14 Ba8 Sb5 84.41(2) 13 13 ?
Sb4 Ba8 Sb5 131.23(2) . 13 ?
Sb9 Ba8 Sb5 93.27(2) 14_556 13 ?
Sb14 Ba8 Sb5 83.04(3) 13 5 ?
Sb4 Ba8 Sb5 86.297(18) . 5 ?
Sb9 Ba8 Sb5 104.44(3) 14_556 5 ?
Sb5 Ba8 Sb5 45.96(2) 13 5 ?
Sb14 Ba8 Cd3 146.331(17) 13 14_556 ?
Sb4 Ba8 Cd3 46.382(19) . 14_556 ?
Sb9 Ba8 Cd3 46.182(17) 14_556 14_556 ?
Sb5 Ba8 Cd3 108.56(3) 13 14_556 ?
Sb5 Ba8 Cd3 84.59(2) 5 14_556 ?
Sb14 Ba8 Ba3 58.684(17) 13 16 ?
Sb4 Ba8 Ba3 55.068(12) . 16 ?
Sb9 Ba8 Ba3 134.13(2) 14_556 16 ?
Sb5 Ba8 Ba3 91.28(2) 13 16 ?
Sb5 Ba8 Ba3 51.48(2) 5 16 ?
Cd3 Ba8 Ba3 89.37(2) 14_556 16 ?
Sb14 Ba8 Ba6 121.38(2) 13 . ?
Sb4 Ba8 Ba6 51.10(2) . . ?
Sb9 Ba8 Ba6 61.158(18) 14_556 . ?
Sb5 Ba8 Ba6 154.130(17) 13 . ?
Sb5 Ba8 Ba6 132.271(19) 5 . ?
Cd3 Ba8 Ba6 51.682(19) 14_556 . ?
Ba3 Ba8 Ba6 103.67(2) 16 . ?
Sb14 Ba8 Ba3 55.658(11) 13 13 ?
Sb4 Ba8 Ba3 156.660(18) . 13 ?
Sb9 Ba8 Ba3 113.722(17) 14_556 13 ?
Sb5 Ba8 Ba3 49.401(18) 13 13 ?
Sb5 Ba8 Ba3 85.885(15) 5 13 ?
Cd3 Ba8 Ba3 153.741(17) 14_556 13 ?
Ba3 Ba8 Ba3 103.576(16) 16 13 ?
Ba6 Ba8 Ba3 141.774(18) . 13 ?
Sb14 Ba8 Ba8 132.318(16) 13 12_655 ?
Sb4 Ba8 Ba8 94.841(11) . 12_655 ?
Sb9 Ba8 Ba8 51.848(16) 14_556 12_655 ?
Sb5 Ba8 Ba8 52.424(15) 13 12_655 ?
Sb5 Ba8 Ba8 53.502(15) 5 12_655 ?
Cd3 Ba8 Ba8 56.938(14) 14_556 12_655 ?
Ba3 Ba8 Ba8 98.618(10) 16 12_655 ?
Ba6 Ba8 Ba8 103.776(10) . 12_655 ?
Ba3 Ba8 Ba8 98.074(9) 13 12_655 ?
Sb14 Ba8 Ba7 116.77(2) 13 . ?
Sb4 Ba8 Ba7 107.209(15) . . ?
Sb9 Ba8 Ba7 52.66(2) 14_556 . ?
Sb5 Ba8 Ba7 112.868(18) 13 . ?
Sb5 Ba8 Ba7 151.922(17) 5 . ?
Cd3 Ba8 Ba7 87.397(16) 14_556 . ?
Ba3 Ba8 Ba7 155.385(17) 16 . ?
Ba6 Ba8 Ba7 56.132(16) . . ?
Ba3 Ba8 Ba7 89.623(12) 13 . ?
Ba8 Ba8 Ba7 99.985(9) 12_655 . ?
Sb14 Ba8 Ba10 113.80(2) 13 13 ?
Sb4 Ba8 Ba10 144.651(17) . 13 ?
Sb9 Ba8 Ba10 55.29(2) 14_556 13 ?
Sb5 Ba8 Ba10 56.85(2) 13 13 ?
Sb5 Ba8 Ba10 98.42(2) 5 13 ?
Cd3 Ba8 Ba10 98.92(2) 14_556 13 ?
Ba3 Ba8 Ba10 148.090(15) 16 13 ?
Ba6 Ba8 Ba10 105.61(2) . 13 ?
Ba3 Ba8 Ba10 58.454(18) 13 13 ?
Ba8 Ba8 Ba10 62.235(11) 12_655 13 ?
Ba7 Ba8 Ba10 56.364(15) . 13 ?
Sb3 Ba9 Sb3 169.24(3) 14_456 7_545 ?
Sb3 Ba9 Sb9 94.106(14) 14_456 . ?
Sb3 Ba9 Sb9 94.106(14) 7_545 . ?
Sb3 Ba9 Sb10 94.293(14) 14_456 . ?
Sb3 Ba9 Sb10 94.293(14) 7_545 . ?
Sb9 Ba9 Sb10 77.24(3) . . ?
Sb3 Ba9 Sb7 88.804(14) 14_456 . ?
Sb3 Ba9 Sb7 88.804(14) 7_545 . ?
Sb9 Ba9 Sb7 62.65(2) . . ?
Sb10 Ba9 Sb7 139.88(2) . . ?
Sb3 Ba9 Ba2 124.51(2) 14_456 . ?
Sb3 Ba9 Ba2 58.043(17) 7_545 . ?
Sb9 Ba9 Ba2 111.83(2) . . ?
Sb10 Ba9 Ba2 49.686(16) . . ?
Sb7 Ba9 Ba2 146.598(13) . . ?
Sb3 Ba9 Ba2 58.044(16) 14_456 12 ?
Sb3 Ba9 Ba2 124.51(2) 7_545 12 ?
Sb9 Ba9 Ba2 111.83(2) . 12 ?
Sb10 Ba9 Ba2 49.686(15) . 12 ?
Sb7 Ba9 Ba2 146.599(14) . 12 ?
Ba2 Ba9 Ba2 66.78(3) . 12 ?
Sb3 Ba9 Ba12 54.084(15) 14_456 3_545 ?
Sb3 Ba9 Ba12 117.04(2) 7_545 3_545 ?
Sb9 Ba9 Ba12 103.12(3) . 3_545 ?
Sb10 Ba9 Ba12 148.370(12) . 3_545 ?
Sb7 Ba9 Ba12 51.282(14) . 3_545 ?
Ba2 Ba9 Ba12 144.85(2) . 3_545 ?
Ba2 Ba9 Ba12 104.01(2) 12 3_545 ?
Sb3 Ba9 Ba12 117.04(2) 14_456 10_556 ?
Sb3 Ba9 Ba12 54.084(15) 7_545 10_556 ?
Sb9 Ba9 Ba12 103.12(3) . 10_556 ?
Sb10 Ba9 Ba12 148.370(12) . 10_556 ?
Sb7 Ba9 Ba12 51.282(14) . 10_556 ?
Ba2 Ba9 Ba12 104.01(2) . 10_556 ?
Ba2 Ba9 Ba12 144.85(2) 12 10_556 ?
Ba12 Ba9 Ba12 63.06(2) 3_545 10_556 ?
Sb3 Ba9 Ba6 141.54(2) 14_456 7_545 ?
Sb3 Ba9 Ba6 49.220(19) 7_545 7_545 ?
Sb9 Ba9 Ba6 58.824(17) . 7_545 ?
Sb10 Ba9 Ba6 55.721(16) . 7_545 ?
Sb7 Ba9 Ba6 99.842(14) . 7_545 ?
Ba2 Ba9 Ba6 56.732(13) . 7_545 ?
Ba2 Ba9 Ba6 104.20(2) 12 7_545 ?
Ba12 Ba9 Ba6 150.782(18) 3_545 7_545 ?
Ba12 Ba9 Ba6 96.80(2) 10_556 7_545 ?
Sb3 Ba9 Ba6 49.220(19) 14_456 14_456 ?
Sb3 Ba9 Ba6 141.54(2) 7_545 14_456 ?
Sb9 Ba9 Ba6 58.824(18) . 14_456 ?
Sb10 Ba9 Ba6 55.721(16) . 14_456 ?
Sb7 Ba9 Ba6 99.842(15) . 14_456 ?
Ba2 Ba9 Ba6 104.20(2) . 14_456 ?
Ba2 Ba9 Ba6 56.734(13) 12 14_456 ?
Ba12 Ba9 Ba6 96.80(2) 3_545 14_456 ?
Ba12 Ba9 Ba6 150.782(18) 10_556 14_456 ?
Ba6 Ba9 Ba6 92.32(3) 7_545 14_456 ?
Sb3 Ba9 Ba7 131.08(2) 14_456 7_545 ?
Sb3 Ba9 Ba7 51.596(16) 7_545 7_545 ?
Sb9 Ba9 Ba7 51.278(14) . 7_545 ?
Sb10 Ba9 Ba7 107.11(2) . 7_545 ?
Sb7 Ba9 Ba7 47.064(16) . 7_545 ?
Ba2 Ba9 Ba7 102.16(2) . 7_545 ?
Ba2 Ba9 Ba7 156.54(2) 12 7_545 ?
Ba12 Ba9 Ba7 96.51(2) 3_545 7_545 ?
Ba12 Ba9 Ba7 56.083(18) 10_556 7_545 ?
Ba6 Ba9 Ba7 54.350(15) 7_545 7_545 ?
Ba6 Ba9 Ba7 110.07(2) 14_456 7_545 ?
Sb1 Ba10 Sb1 158.98(3) . 12 ?
Sb1 Ba10 Sb8 85.024(13) . . ?
Sb1 Ba10 Sb8 85.024(14) 12 . ?
Sb1 Ba10 Cd1 114.67(2) . 12 ?
Sb1 Ba10 Cd1 46.409(14) 12 12 ?
Sb8 Ba10 Cd1 48.103(19) . 12 ?
Sb1 Ba10 Cd1 46.410(14) . . ?
Sb1 Ba10 Cd1 114.67(2) 12 . ?
Sb8 Ba10 Cd1 48.103(19) . . ?
Cd1 Ba10 Cd1 68.51(3) 12 . ?
Sb1 Ba10 Sb11 79.581(13) . . ?
Sb1 Ba10 Sb11 79.580(13) 12 . ?
Sb8 Ba10 Sb11 69.01(3) . . ?
Cd1 Ba10 Sb11 46.058(18) 12 . ?
Cd1 Ba10 Sb11 46.057(18) . . ?
Sb1 Ba10 Sb9 99.297(13) . 2_554 ?
Sb1 Ba10 Sb9 99.297(13) 12 2_554 ?
Sb8 Ba10 Sb9 146.04(3) . 2_554 ?
Cd1 Ba10 Sb9 145.686(15) 12 2_554 ?
Cd1 Ba10 Sb9 145.687(15) . 2_554 ?
Sb11 Ba10 Sb9 144.94(3) . 2_554 ?
Sb1 Ba10 Sb7 90.394(14) . 2_554 ?
Sb1 Ba10 Sb7 90.394(14) 12 2_554 ?
Sb8 Ba10 Sb7 153.76(2) . 2_554 ?
Cd1 Ba10 Sb7 112.56(2) 12 2_554 ?
Cd1 Ba10 Sb7 112.56(2) . 2_554 ?
Sb11 Ba10 Sb7 84.75(3) . 2_554 ?
Sb9 Ba10 Sb7 60.19(2) 2_554 2_554 ?
Sb1 Ba10 Sb5 96.318(13) . . ?
Sb1 Ba10 Sb5 96.318(13) 12 . ?
Sb8 Ba10 Sb5 65.51(2) . . ?
Cd1 Ba10 Sb5 99.582(17) 12 . ?
Cd1 Ba10 Sb5 99.582(17) . . ?
Sb11 Ba10 Sb5 134.52(2) . . ?
Sb9 Ba10 Sb5 80.530(18) 2_554 . ?
Sb7 Ba10 Sb5 140.72(3) 2_554 . ?
Sb1 Ba10 Ba7 137.33(2) . 8_455 ?
Sb1 Ba10 Ba7 52.699(18) 12 8_455 ?
Sb8 Ba10 Ba7 136.991(14) . 8_455 ?
Cd1 Ba10 Ba7 96.20(2) 12 8_455 ?
Cd1 Ba10 Ba7 151.15(2) . 8_455 ?
Sb11 Ba10 Ba7 105.60(2) . 8_455 ?
Sb9 Ba10 Ba7 52.357(15) 2_554 8_455 ?
Sb7 Ba10 Ba7 49.264(13) 2_554 8_455 ?
Sb5 Ba10 Ba7 107.232(17) . 8_455 ?
Sb1 Ba10 Ba7 52.699(18) . 13 ?
Sb1 Ba10 Ba7 137.33(2) 12 13 ?
Sb8 Ba10 Ba7 136.991(14) . 13 ?
Cd1 Ba10 Ba7 151.15(2) 12 13 ?
Cd1 Ba10 Ba7 96.20(2) . 13 ?
Sb11 Ba10 Ba7 105.60(2) . 13 ?
Sb9 Ba10 Ba7 52.357(15) 2_554 13 ?
Sb7 Ba10 Ba7 49.264(13) 2_554 13 ?
Sb5 Ba10 Ba7 107.232(17) . 13 ?
Ba7 Ba10 Ba7 86.01(3) 8_455 13 ?
Sb1 Ba10 Ba3 53.202(18) . . ?
Sb1 Ba10 Ba3 130.15(2) 12 . ?
Sb8 Ba10 Ba3 52.217(14) . . ?
Cd1 Ba10 Ba3 100.24(2) 12 . ?
Cd1 Ba10 Ba3 57.703(16) . . ?
Sb11 Ba10 Ba3 102.89(2) . . ?
Sb9 Ba10 Ba3 104.092(17) 2_554 . ?
Sb7 Ba10 Ba3 139.382(14) 2_554 . ?
Sb5 Ba10 Ba3 46.746(16) . . ?
Ba7 Ba10 Ba3 151.146(19) 8_455 . ?
Ba7 Ba10 Ba3 90.75(2) 13 . ?
Cd1 Ba11 Cd1 73.61(3) . 12 ?
Cd1 Ba11 Sb2 51.182(16) . . ?
Cd1 Ba11 Sb2 124.79(2) 12 . ?
Cd1 Ba11 Sb2 124.79(2) . 12 ?
Cd1 Ba11 Sb2 51.184(16) 12 12 ?
Sb2 Ba11 Sb2 175.92(2) . 12 ?
Cd1 Ba11 Sb8 49.761(19) . . ?
Cd1 Ba11 Sb8 49.759(19) 12 . ?
Sb2 Ba11 Sb8 88.187(13) . . ?
Sb2 Ba11 Sb8 88.187(13) 12 . ?
Cd1 Ba11 Sb11 48.786(18) . . ?
Cd1 Ba11 Sb11 48.786(18) 12 . ?
Sb2 Ba11 Sb11 88.525(13) . . ?
Sb2 Ba11 Sb11 88.525(13) 12 . ?
Sb8 Ba11 Sb11 70.84(3) . . ?
Cd1 Ba11 Sb10 143.120(16) . . ?
Cd1 Ba11 Sb10 143.121(16) 12 . ?
Sb2 Ba11 Sb10 91.997(12) . . ?
Sb2 Ba11 Sb10 91.997(12) 12 . ?
Sb8 Ba11 Sb10 141.24(3) . . ?
Sb11 Ba11 Sb10 147.92(3) . . ?
Cd1 Ba11 Sb12 92.814(17) . . ?
Cd1 Ba11 Sb12 92.814(17) 12 . ?
Sb2 Ba11 Sb12 90.442(13) . . ?
Sb2 Ba11 Sb12 90.443(13) 12 . ?
Sb8 Ba11 Sb12 129.73(2) . . ?
Sb11 Ba11 Sb12 58.89(2) . . ?
Sb10 Ba11 Sb12 89.026(19) . . ?
Cd1 Ba11 Sb6 98.342(18) . . ?
Cd1 Ba11 Sb6 98.341(18) 12 . ?
Sb2 Ba11 Sb6 90.051(13) . . ?
Sb2 Ba11 Sb6 90.050(13) 12 . ?
Sb8 Ba11 Sb6 64.22(2) . . ?
Sb11 Ba11 Sb6 135.06(2) . . ?
Sb10 Ba11 Sb6 77.020(18) . . ?
Sb12 Ba11 Sb6 166.05(2) . . ?
Cd1 Ba11 Ba1 145.76(2) . 12 ?
Cd1 Ba11 Ba1 101.23(2) 12 12 ?
Sb2 Ba11 Ba1 123.55(2) . 12 ?
Sb2 Ba11 Ba1 59.898(15) 12 12 ?
Sb8 Ba11 Ba1 147.801(12) . 12 ?
Sb11 Ba11 Ba1 101.89(3) . 12 ?
Sb10 Ba11 Ba1 52.243(16) . 12 ?
Sb12 Ba11 Ba1 53.180(15) . 12 ?
Sb6 Ba11 Ba1 115.87(2) . 12 ?
Cd1 Ba11 Ba1 101.23(2) . . ?
Cd1 Ba11 Ba1 145.76(2) 12 . ?
Sb2 Ba11 Ba1 59.896(15) . . ?
Sb2 Ba11 Ba1 123.55(2) 12 . ?
Sb8 Ba11 Ba1 147.800(13) . . ?
Sb11 Ba11 Ba1 101.89(3) . . ?
Sb10 Ba11 Ba1 52.242(16) . . ?
Sb12 Ba11 Ba1 53.181(15) . . ?
Sb6 Ba11 Ba1 115.87(2) . . ?
Ba1 Ba11 Ba1 63.66(2) 12 . ?
Cd1 Ba11 Ba2 146.69(2) . 12 ?
Cd1 Ba11 Ba2 101.28(2) 12 12 ?
Sb2 Ba11 Ba2 123.61(2) . 12 ?
Sb2 Ba11 Ba2 59.044(16) 12 12 ?
Sb8 Ba11 Ba2 101.31(3) . 12 ?
Sb11 Ba11 Ba2 147.252(13) . 12 ?
Sb10 Ba11 Ba2 48.114(15) . 12 ?
Sb12 Ba11 Ba2 120.465(19) . 12 ?
Sb6 Ba11 Ba2 49.069(13) . 12 ?
Ba1 Ba11 Ba2 67.34(2) 12 12 ?
Ba1 Ba11 Ba2 100.27(3) . 12 ?
Sb14 Ba12 Sb11 173.692(18) 13 . ?
Sb14 Ba12 Sb1 90.252(18) 13 . ?
Sb11 Ba12 Sb1 83.44(2) . . ?
Sb14 Ba12 Sb3 90.71(2) 13 16 ?
Sb11 Ba12 Sb3 93.08(2) . 16 ?
Sb1 Ba12 Sb3 127.44(2) . 16 ?
Sb14 Ba12 Sb7 87.16(2) 13 10_566 ?
Sb11 Ba12 Sb7 97.84(2) . 10_566 ?
Sb1 Ba12 Sb7 142.09(2) . 10_566 ?
Sb3 Ba12 Sb7 90.42(3) 16 10_566 ?
Sb14 Ba12 Sb7 86.66(3) 13 2_554 ?
Sb11 Ba12 Sb7 93.96(3) . 2_554 ?
Sb1 Ba12 Sb7 95.316(19) . 2_554 ?
Sb3 Ba12 Sb7 137.19(2) 16 2_554 ?
Sb7 Ba12 Sb7 46.78(2) 10_566 2_554 ?
Sb14 Ba12 Ba7 58.199(17) 13 13 ?
Sb11 Ba12 Ba7 117.48(2) . 13 ?
Sb1 Ba12 Ba7 55.131(15) . 13 ?
Sb3 Ba12 Ba7 148.544(18) 16 13 ?
Sb7 Ba12 Ba7 92.45(2) 10_566 13 ?
Sb7 Ba12 Ba7 53.086(19) 2_554 13 ?
Sb14 Ba12 Ba5 122.20(2) 13 . ?
Sb11 Ba12 Ba5 57.33(2) . . ?
Sb1 Ba12 Ba5 85.033(14) . . ?
Sb3 Ba12 Ba5 51.412(17) 16 . ?
Sb7 Ba12 Ba5 127.495(18) 10_566 . ?
Sb7 Ba12 Ba5 151.131(17) 2_554 . ?
Ba7 Ba12 Ba5 139.48(2) 13 . ?
Sb14 Ba12 Ba7 56.554(9) 13 16 ?
Sb11 Ba12 Ba7 129.692(17) . 16 ?
Sb1 Ba12 Ba7 146.14(2) . 16 ?
Sb3 Ba12 Ba7 54.64(2) 16 16 ?
Sb7 Ba12 Ba7 51.907(18) 10_566 16 ?
Sb7 Ba12 Ba7 89.672(17) 2_554 16 ?
Ba7 Ba12 Ba7 104.46(2) 13 16 ?
Ba5 Ba12 Ba7 106.043(14) . 16 ?
Sb14 Ba12 Ba9 121.11(2) 13 10_566 ?
Sb11 Ba12 Ba9 65.03(2) . 10_566 ?
Sb1 Ba12 Ba9 146.268(18) . 10_566 ?
Sb3 Ba12 Ba9 48.147(18) 16 10_566 ?
Sb7 Ba12 Ba9 59.10(2) 10_566 10_566 ?
Sb7 Ba12 Ba9 98.37(2) 2_554 10_566 ?
Ba7 Ba12 Ba9 150.742(15) 13 10_566 ?
Ba5 Ba12 Ba9 68.392(17) . 10_566 ?
Ba7 Ba12 Ba9 64.80(2) 16 10_566 ?
Sb14 Ba12 Ba10 119.420(17) 13 . ?
Sb11 Ba12 Ba10 56.281(19) . . ?
Sb1 Ba12 Ba10 51.90(2) . . ?
Sb3 Ba12 Ba10 149.044(18) 16 . ?
Sb7 Ba12 Ba10 97.54(3) 10_566 . ?
Sb7 Ba12 Ba10 58.138(16) 2_554 . ?
Ba7 Ba12 Ba10 61.264(15) 13 . ?
Ba5 Ba12 Ba10 101.881(14) . . ?
Ba7 Ba12 Ba10 147.529(17) 16 . ?
Ba9 Ba12 Ba10 112.24(2) 10_566 . ?
Sb14 Ba12 Ba12 133.671(16) 13 12 ?
Sb11 Ba12 Ba12 49.642(15) . 12 ?
Sb1 Ba12 Ba12 110.096(13) . 12 ?
Sb3 Ba12 Ba12 106.539(12) 16 12 ?
Sb7 Ba12 Ba12 51.080(14) 10_566 12 ?
Sb7 Ba12 Ba12 51.472(15) 2_554 12 ?
Ba7 Ba12 Ba12 99.496(10) 13 12 ?
Ba5 Ba12 Ba12 101.288(10) . 12 ?
Ba7 Ba12 Ba12 99.164(9) 16 12 ?
Ba9 Ba12 Ba12 58.473(13) 10_566 12 ?
Ba10 Ba12 Ba12 58.820(13) . 12 ?
Sb1 Cd1 Sb11 106.95(3) . . ?
Sb1 Cd1 Sb8 109.27(3) . . ?
Sb11 Cd1 Sb8 88.82(3) . . ?
Sb1 Cd1 Sb2 124.13(3) . . ?
Sb11 Cd1 Sb2 112.30(2) . . ?
Sb8 Cd1 Sb2 109.66(2) . . ?
Sb1 Cd1 Ba11 171.40(2) . . ?
Sb11 Cd1 Ba11 66.93(2) . . ?
Sb8 Cd1 Ba11 65.50(2) . . ?
Sb2 Cd1 Ba11 64.46(3) . . ?
Sb1 Cd1 Ba5 104.19(2) . . ?
Sb11 Cd1 Ba5 66.52(2) . . ?
Sb8 Cd1 Ba5 143.09(2) . . ?
Sb2 Cd1 Ba5 60.666(18) . . ?
Ba11 Cd1 Ba5 79.296(19) . . ?
Sb1 Cd1 Ba6 63.045(19) . . ?
Sb11 Cd1 Ba6 137.72(2) . . ?
Sb8 Cd1 Ba6 133.43(2) . . ?
Sb2 Cd1 Ba6 61.124(17) . . ?
Ba11 Cd1 Ba6 125.56(2) . . ?
Ba5 Cd1 Ba6 76.167(15) . . ?
Sb1 Cd1 Ba10 62.75(3) . . ?
Sb11 Cd1 Ba10 67.32(2) . . ?
Sb8 Cd1 Ba10 62.07(2) . . ?
Sb2 Cd1 Ba10 171.56(2) . . ?
Ba11 Cd1 Ba10 108.74(3) . . ?
Ba5 Cd1 Ba10 124.45(2) . . ?
Ba6 Cd1 Ba10 125.27(2) . . ?
Sb1 Cd1 Ba4 109.91(2) . . ?
Sb11 Cd1 Ba4 139.33(2) . . ?
Sb8 Cd1 Ba4 63.32(2) . . ?
Sb2 Cd1 Ba4 57.987(17) . . ?
Ba11 Cd1 Ba4 74.41(2) . . ?
Ba5 Cd1 Ba4 118.64(3) . . ?
Ba6 Cd1 Ba4 76.192(14) . . ?
Ba10 Cd1 Ba4 116.33(2) . . ?
Sb1 Cd1 Ba3 61.407(18) . . ?
Sb11 Cd1 Ba3 134.27(2) . . ?
Sb8 Cd1 Ba3 59.66(2) . . ?
Sb2 Cd1 Ba3 109.39(2) . . ?
Ba11 Cd1 Ba3 117.95(2) . . ?
Ba5 Cd1 Ba3 155.76(2) . . ?
Ba6 Cd1 Ba3 79.763(14) . . ?
Ba10 Cd1 Ba3 68.644(17) . . ?
Ba4 Cd1 Ba3 56.92(2) . . ?
Sb4 Cd2 Sb4 118.57(4) 5_445 16_545 ?
Sb4 Cd2 Sb8 113.90(2) 5_445 . ?
Sb4 Cd2 Sb8 113.90(2) 16_545 . ?
Sb4 Cd2 Sb6 109.75(2) 5_445 . ?
Sb4 Cd2 Sb6 109.75(2) 16_545 . ?
Sb8 Cd2 Sb6 86.10(3) . . ?
Sb4 Cd2 Cd3 59.792(19) 5_445 10_556 ?
Sb4 Cd2 Cd3 59.79(2) 16_545 10_556 ?
Sb8 Cd2 Cd3 152.38(4) . 10_556 ?
Sb6 Cd2 Cd3 121.52(3) . 10_556 ?
Sb4 Cd2 Ba4 172.30(3) 5_445 . ?
Sb4 Cd2 Ba4 65.10(2) 16_545 . ?
Sb8 Cd2 Ba4 68.306(19) . . ?
Sb6 Cd2 Ba4 62.683(16) . . ?
Cd3 Cd2 Ba4 121.943(17) 10_556 . ?
Sb4 Cd2 Ba4 65.10(2) 5_445 12 ?
Sb4 Cd2 Ba4 172.30(3) 16_545 12 ?
Sb8 Cd2 Ba4 68.306(19) . 12 ?
Sb6 Cd2 Ba4 62.682(16) . 12 ?
Cd3 Cd2 Ba4 121.943(17) 10_556 12 ?
Ba4 Cd2 Ba4 110.41(3) . 12 ?
Sb4 Cd2 Ba3 57.66(2) 5_445 12 ?
Sb4 Cd2 Ba3 129.43(3) 16_545 12 ?
Sb8 Cd2 Ba3 58.665(16) . 12 ?
Sb6 Cd2 Ba3 118.66(2) . 12 ?
Cd3 Cd2 Ba3 102.80(2) 10_556 12 ?
Ba4 Cd2 Ba3 126.23(3) . 12 ?
Ba4 Cd2 Ba3 58.22(2) 12 12 ?
Sb4 Cd2 Ba3 129.43(3) 5_445 . ?
Sb4 Cd2 Ba3 57.66(2) 16_545 . ?
Sb8 Cd2 Ba3 58.665(16) . . ?
Sb6 Cd2 Ba3 118.66(2) . . ?
Cd3 Cd2 Ba3 102.80(2) 10_556 . ?
Ba4 Cd2 Ba3 58.22(2) . . ?
Ba4 Cd2 Ba3 126.23(3) 12 . ?
Ba3 Cd2 Ba3 85.77(3) 12 . ?
Sb10 Cd3 Sb9 104.02(4) . . ?
Sb10 Cd3 Sb4 108.08(2) . 7_545 ?
Sb9 Cd3 Sb4 112.16(2) . 7_545 ?
Sb10 Cd3 Sb4 108.08(2) . 14_456 ?
Sb9 Cd3 Sb4 112.16(2) . 14_456 ?
Sb4 Cd3 Sb4 111.88(4) 7_545 14_456 ?
Sb10 Cd3 Cd2 114.95(4) . 10_566 ?
Sb9 Cd3 Cd2 141.04(3) . 10_566 ?
Sb4 Cd3 Cd2 56.38(2) 7_545 10_566 ?
Sb4 Cd3 Cd2 56.385(19) 14_456 10_566 ?
Sb10 Cd3 Ba6 72.431(18) . 14_456 ?
Sb9 Cd3 Ba6 74.370(18) . 14_456 ?
Sb4 Cd3 Ba6 172.72(3) 7_545 14_456 ?
Sb4 Cd3 Ba6 61.62(3) 14_456 14_456 ?
Cd2 Cd3 Ba6 116.579(17) 10_566 14_456 ?
Sb10 Cd3 Ba6 72.431(17) . 7_545 ?
Sb9 Cd3 Ba6 74.370(18) . 7_545 ?
Sb4 Cd3 Ba6 61.62(3) 7_545 7_545 ?
Sb4 Cd3 Ba6 172.72(3) 14_456 7_545 ?
Cd2 Cd3 Ba6 116.579(17) 10_566 7_545 ?
Ba6 Cd3 Ba6 124.64(3) 14_456 7_545 ?
Sb10 Cd3 Ba8 139.76(2) . 7_545 ?
Sb9 Cd3 Ba8 58.63(2) . 7_545 ?
Sb4 Cd3 Ba8 58.163(18) 7_545 7_545 ?
Sb4 Cd3 Ba8 112.11(3) 14_456 7_545 ?
Cd2 Cd3 Ba8 89.53(2) 10_566 7_545 ?
Ba6 Cd3 Ba8 126.26(2) 14_456 7_545 ?
Ba6 Cd3 Ba8 67.983(17) 7_545 7_545 ?
Sb10 Cd3 Ba8 139.76(2) . 14_456 ?
Sb9 Cd3 Ba8 58.63(2) . 14_456 ?
Sb4 Cd3 Ba8 112.11(3) 7_545 14_456 ?
Sb4 Cd3 Ba8 58.163(18) 14_456 14_456 ?
Cd2 Cd3 Ba8 89.53(2) 10_566 14_456 ?
Ba6 Cd3 Ba8 67.983(17) 14_456 14_456 ?
Ba6 Cd3 Ba8 126.26(2) 7_545 14_456 ?
Ba8 Cd3 Ba8 66.13(3) 7_545 14_456 ?
Cd1 Sb1 Ba7 125.63(2) . . ?
Cd1 Sb1 Ba6 70.16(3) . . ?
Ba7 Sb1 Ba6 71.23(2) . . ?
Cd1 Sb1 Ba7 138.03(3) . 13 ?
Ba7 Sb1 Ba7 94.64(2) . 13 ?
Ba6 Sb1 Ba7 143.77(2) . 13 ?
Cd1 Sb1 Ba10 70.84(2) . . ?
Ba7 Sb1 Ba10 129.14(2) . . ?
Ba6 Sb1 Ba10 140.25(2) . . ?
Ba7 Sb1 Ba10 74.537(16) 13 . ?
Cd1 Sb1 Ba12 79.782(18) . . ?
Ba7 Sb1 Ba12 146.886(18) . . ?
Ba6 Sb1 Ba12 104.342(18) . . ?
Ba7 Sb1 Ba12 69.234(16) 13 . ?
Ba10 Sb1 Ba12 75.816(19) . . ?
Cd1 Sb1 Ba3 73.983(17) . . ?
Ba7 Sb1 Ba3 67.35(2) . . ?
Ba6 Sb1 Ba3 87.228(16) . . ?
Ba7 Sb1 Ba3 118.712(17) 13 . ?
Ba10 Sb1 Ba3 74.974(16) . . ?
Ba12 Sb1 Ba3 145.71(2) . . ?
Cd1 Sb2 Ba4 72.481(18) . . ?
Cd1 Sb2 Ba5 68.331(17) . . ?
Ba4 Sb2 Ba5 140.80(2) . . ?
Cd1 Sb2 Ba6 68.91(3) . . ?
Ba4 Sb2 Ba6 84.978(17) . . ?
Ba5 Sb2 Ba6 82.200(17) . . ?
Cd1 Sb2 Ba11 64.36(2) . . ?
Ba4 Sb2 Ba11 79.899(17) . . ?
Ba5 Sb2 Ba11 82.381(17) . . ?
Ba6 Sb2 Ba11 133.24(2) . . ?
Cd1 Sb2 Ba1 118.19(2) . . ?
Ba4 Sb2 Ba1 133.636(19) . . ?
Ba5 Sb2 Ba1 68.17(2) . . ?
Ba6 Sb2 Ba1 141.35(2) . . ?
Ba11 Sb2 Ba1 68.272(16) . . ?
Cd1 Sb2 Ba2 120.96(2) . 7_545 ?
Ba4 Sb2 Ba2 67.06(2) . 7_545 ?
Ba5 Sb2 Ba2 137.095(19) . 7_545 ?
Ba6 Sb2 Ba2 66.48(2) . 7_545 ?
Ba11 Sb2 Ba2 140.49(2) . 7_545 ?
Ba1 Sb2 Ba2 120.84(2) . 7_545 ?
Cd1 Sb2 Ba2 121.83(2) . . ?
Ba4 Sb2 Ba2 63.75(2) . . ?
Ba5 Sb2 Ba2 140.337(18) . . ?
Ba6 Sb2 Ba2 137.30(2) . . ?
Ba11 Sb2 Ba2 71.672(16) . . ?
Ba1 Sb2 Ba2 74.47(2) . . ?
Ba2 Sb2 Ba2 74.52(2) 7_545 . ?
Ba9 Sb3 Ba6 82.500(18) 14_556 . ?
Ba9 Sb3 Ba5 90.649(19) 14_556 16_545 ?
Ba6 Sb3 Ba5 143.09(2) . 16_545 ?
Ba9 Sb3 Ba3 150.16(2) 14_556 . ?
Ba6 Sb3 Ba3 93.669(16) . . ?
Ba5 Sb3 Ba3 108.892(19) 16_545 . ?
Ba9 Sb3 Ba4 143.25(2) 14_556 . ?
Ba6 Sb3 Ba4 86.263(15) . . ?
Ba5 Sb3 Ba4 77.803(18) 16_545 . ?
Ba3 Sb3 Ba4 65.18(3) . . ?
Ba9 Sb3 Ba12 77.770(19) 14_556 16_545 ?
Ba6 Sb3 Ba12 139.90(2) . 16_545 ?
Ba5 Sb3 Ba12 72.08(3) 16_545 16_545 ?
Ba3 Sb3 Ba12 86.85(2) . 16_545 ?
Ba4 Sb3 Ba12 128.97(2) . 16_545 ?
Ba9 Sb3 Ba7 82.611(17) 14_556 . ?
Ba6 Sb3 Ba7 71.930(18) . . ?
Ba5 Sb3 Ba7 143.236(18) 16_545 . ?
Ba3 Sb3 Ba7 68.178(18) . . ?
Ba4 Sb3 Ba7 126.51(2) . . ?
Ba12 Sb3 Ba7 71.16(2) 16_545 . ?
Ba9 Sb3 Ba2 74.451(17) 14_556 7_545 ?
Ba6 Sb3 Ba2 70.333(14) . 7_545 ?
Ba5 Sb3 Ba2 72.88(2) 16_545 7_545 ?
Ba3 Sb3 Ba2 132.066(18) . 7_545 ?
Ba4 Sb3 Ba2 68.82(2) . 7_545 ?
Ba12 Sb3 Ba2 134.452(19) 16_545 7_545 ?
Ba7 Sb3 Ba2 137.80(2) . 7_545 ?
Cd2 Sb4 Cd3 63.82(3) 5 14_556 ?
Cd2 Sb4 Ba6 130.06(2) 5 . ?
Cd3 Sb4 Ba6 68.14(2) 14_556 . ?
Cd2 Sb4 Ba8 103.75(2) 5 . ?
Cd3 Sb4 Ba8 75.46(2) 14_556 . ?
Ba6 Sb4 Ba8 75.956(16) . . ?
Cd2 Sb4 Ba4 66.91(2) 5 16 ?
Cd3 Sb4 Ba4 127.39(2) 14_556 16 ?
Ba6 Sb4 Ba4 145.11(2) . 16 ?
Ba8 Sb4 Ba4 134.790(18) . 16 ?
Cd2 Sb4 Ba3 78.75(2) 5 16 ?
Cd3 Sb4 Ba3 120.36(2) 14_556 16 ?
Ba6 Sb4 Ba3 140.51(2) . 16 ?
Ba8 Sb4 Ba3 70.36(2) . 16 ?
Ba4 Sb4 Ba3 64.45(3) 16 16 ?
Cd2 Sb4 Ba1 82.54(2) 5 7_545 ?
Cd3 Sb4 Ba1 80.84(2) 14_556 7_545 ?
Ba6 Sb4 Ba1 77.167(16) . 7_545 ?
Ba8 Sb4 Ba1 149.22(2) . 7_545 ?
Ba4 Sb4 Ba1 75.63(2) 16 7_545 ?
Ba3 Sb4 Ba1 139.902(19) 16 7_545 ?
Cd2 Sb4 Ba5 136.05(3) 5 . ?
Cd3 Sb4 Ba5 140.88(2) 14_556 . ?
Ba6 Sb4 Ba5 78.686(15) . . ?
Ba8 Sb4 Ba5 116.628(18) . . ?
Ba4 Sb4 Ba5 72.372(15) 16 . ?
Ba3 Sb4 Ba5 98.356(17) 16 . ?
Ba1 Sb4 Ba5 71.849(17) 7_545 . ?
Sb5 Sb5 Ba3 123.434(17) 9 12 ?
Sb5 Sb5 Ba3 123.433(17) 9 . ?
Ba3 Sb5 Ba3 111.60(3) 12 . ?
Sb5 Sb5 Ba8 68.70(3) 9 8_455 ?
Ba3 Sb5 Ba8 76.95(2) 12 8_455 ?
Ba3 Sb5 Ba8 141.52(3) . 8_455 ?
Sb5 Sb5 Ba8 68.70(3) 9 13 ?
Ba3 Sb5 Ba8 141.52(3) 12 13 ?
Ba3 Sb5 Ba8 76.95(2) . 13 ?
Ba8 Sb5 Ba8 75.15(3) 8_455 13 ?
Sb5 Sb5 Ba8 65.34(3) 9 5_445 ?
Ba3 Sb5 Ba8 70.21(2) 12 5_445 ?
Ba3 Sb5 Ba8 130.19(2) . 5_445 ?
Ba8 Sb5 Ba8 88.27(2) 8_455 5_445 ?
Ba8 Sb5 Ba8 134.04(2) 13 5_445 ?
Sb5 Sb5 Ba8 65.34(3) 9 16_545 ?
Ba3 Sb5 Ba8 130.19(2) 12 16_545 ?
Ba3 Sb5 Ba8 70.21(2) . 16_545 ?
Ba8 Sb5 Ba8 134.04(2) 8_455 16_545 ?
Ba8 Sb5 Ba8 88.27(2) 13 16_545 ?
Ba8 Sb5 Ba8 72.99(3) 5_445 16_545 ?
Sb5 Sb5 Ba10 134.27(4) 9 . ?
Ba3 Sb5 Ba10 72.251(16) 12 . ?
Ba3 Sb5 Ba10 72.250(16) . . ?
Ba8 Sb5 Ba10 75.465(19) 8_455 . ?
Ba8 Sb5 Ba10 75.465(18) 13 . ?
Ba8 Sb5 Ba10 141.564(16) 5_445 . ?
Ba8 Sb5 Ba10 141.564(16) 16_545 . ?
Sb12 Sb6 Cd2 128.35(4) 10_556 . ?
Sb12 Sb6 Ba4 121.585(16) 10_556 12 ?
Cd2 Sb6 Ba4 66.271(18) . 12 ?
Sb12 Sb6 Ba4 121.587(16) 10_556 . ?
Cd2 Sb6 Ba4 66.269(18) . . ?
Ba4 Sb6 Ba4 115.58(3) 12 . ?
Sb12 Sb6 Ba2 73.67(2) 10_556 12 ?
Cd2 Sb6 Ba2 135.363(17) . 12 ?
Ba4 Sb6 Ba2 69.28(2) 12 12 ?
Ba4 Sb6 Ba2 141.60(3) . 12 ?
Sb12 Sb6 Ba2 73.67(2) 10_556 . ?
Cd2 Sb6 Ba2 135.364(17) . . ?
Ba4 Sb6 Ba2 141.60(3) 12 . ?
Ba4 Sb6 Ba2 69.28(2) . . ?
Ba2 Sb6 Ba2 84.48(3) 12 . ?
Sb12 Sb6 Ba1 63.58(2) 10_556 3_545 ?
Cd2 Sb6 Ba1 74.56(2) . 3_545 ?
Ba4 Sb6 Ba1 71.537(19) 12 3_545 ?
Ba4 Sb6 Ba1 130.26(2) . 3_545 ?
Ba2 Sb6 Ba1 88.04(2) 12 3_545 ?
Ba2 Sb6 Ba1 136.97(2) . 3_545 ?
Sb12 Sb6 Ba1 63.58(2) 10_556 10_556 ?
Cd2 Sb6 Ba1 74.56(2) . 10_556 ?
Ba4 Sb6 Ba1 130.26(2) 12 10_556 ?
Ba4 Sb6 Ba1 71.54(2) . 10_556 ?
Ba2 Sb6 Ba1 136.97(2) 12 10_556 ?
Ba2 Sb6 Ba1 88.04(2) . 10_556 ?
Ba1 Sb6 Ba1 69.37(3) 3_545 10_556 ?
Sb12 Sb6 Ba11 132.88(3) 10_556 . ?
Cd2 Sb6 Ba11 98.77(3) . . ?
Ba4 Sb6 Ba11 73.500(15) 12 . ?
Ba4 Sb6 Ba11 73.500(15) . . ?
Ba2 Sb6 Ba11 71.910(19) 12 . ?
Ba2 Sb6 Ba11 71.910(19) . . ?
Ba1 Sb6 Ba11 144.049(15) 3_545 . ?
Ba1 Sb6 Ba11 144.049(16) 10_556 . ?
Sb7 Sb7 Ba7 121.667(16) 9_556 7_545 ?
Sb7 Sb7 Ba7 121.667(17) 9_556 14_456 ?
Ba7 Sb7 Ba7 116.34(3) 7_545 14_456 ?
Sb7 Sb7 Ba12 67.17(3) 9_556 3_545 ?
Ba7 Sb7 Ba12 140.49(2) 7_545 3_545 ?
Ba7 Sb7 Ba12 72.79(2) 14_456 3_545 ?
Sb7 Sb7 Ba12 67.17(3) 9_556 10_556 ?
Ba7 Sb7 Ba12 72.79(2) 7_545 10_556 ?
Ba7 Sb7 Ba12 140.49(2) 14_456 10_556 ?
Ba12 Sb7 Ba12 77.84(3) 3_545 10_556 ?
Sb7 Sb7 Ba12 66.05(2) 9_556 11_566 ?
Ba7 Sb7 Ba12 69.52(2) 7_545 11_566 ?
Ba7 Sb7 Ba12 135.12(2) 14_456 11_566 ?
Ba12 Sb7 Ba12 133.22(2) 3_545 11_566 ?
Ba12 Sb7 Ba12 84.38(2) 10_556 11_566 ?
Sb7 Sb7 Ba12 66.05(2) 9_556 2 ?
Ba7 Sb7 Ba12 135.12(2) 7_545 2 ?
Ba7 Sb7 Ba12 69.52(2) 14_456 2 ?
Ba12 Sb7 Ba12 84.38(2) 3_545 2 ?
Ba12 Sb7 Ba12 133.22(2) 10_556 2 ?
Ba12 Sb7 Ba12 77.06(3) 11_566 2 ?
Sb7 Sb7 Ba10 123.28(4) 9_556 2 ?
Ba7 Sb7 Ba10 70.709(18) 7_545 2 ?
Ba7 Sb7 Ba10 70.709(19) 14_456 2 ?
Ba12 Sb7 Ba10 140.958(15) 3_545 2 ?
Ba12 Sb7 Ba10 140.958(15) 10_556 2 ?
Ba12 Sb7 Ba10 70.35(2) 11_566 2 ?
Ba12 Sb7 Ba10 70.35(2) 2 2 ?
Sb7 Sb7 Ba9 123.49(4) 9_556 . ?
Ba7 Sb7 Ba9 75.670(15) 7_545 . ?
Ba7 Sb7 Ba9 75.670(15) 14_456 . ?
Ba12 Sb7 Ba9 69.613(19) 3_545 . ?
Ba12 Sb7 Ba9 69.613(19) 10_556 . ?
Ba12 Sb7 Ba9 141.416(15) 11_566 . ?
Ba12 Sb7 Ba9 141.416(16) 2 . ?
Ba10 Sb7 Ba9 113.23(3) 2 . ?
Cd2 Sb8 Cd1 132.52(2) . 12 ?
Cd2 Sb8 Cd1 132.52(2) . . ?
Cd1 Sb8 Cd1 90.44(4) 12 . ?
Cd2 Sb8 Ba10 135.69(3) . . ?
Cd1 Sb8 Ba10 69.82(2) 12 . ?
Cd1 Sb8 Ba10 69.83(2) . . ?
Cd2 Sb8 Ba3 76.75(2) . 12 ?
Cd1 Sb8 Ba3 73.82(2) 12 12 ?
Cd1 Sb8 Ba3 145.31(3) . 12 ?
Ba10 Sb8 Ba3 75.71(2) . 12 ?
Cd2 Sb8 Ba3 76.75(2) . . ?
Cd1 Sb8 Ba3 145.30(3) 12 . ?
Cd1 Sb8 Ba3 73.82(2) . . ?
Ba10 Sb8 Ba3 75.71(2) . . ?
Ba3 Sb8 Ba3 101.70(3) 12 . ?
Cd2 Sb8 Ba11 110.90(3) . . ?
Cd1 Sb8 Ba11 64.75(2) 12 . ?
Cd1 Sb8 Ba11 64.74(2) . . ?
Ba10 Sb8 Ba11 113.41(3) . . ?
Ba3 Sb8 Ba11 129.149(15) 12 . ?
Ba3 Sb8 Ba11 129.149(15) . . ?
Cd2 Sb8 Ba4 63.717(16) . . ?
Cd1 Sb8 Ba4 141.12(3) 12 . ?
Cd1 Sb8 Ba4 69.73(2) . . ?
Ba10 Sb8 Ba4 127.584(15) . . ?
Ba3 Sb8 Ba4 139.44(3) 12 . ?
Ba3 Sb8 Ba4 62.02(2) . . ?
Ba11 Sb8 Ba4 76.47(2) . . ?
Cd2 Sb8 Ba4 63.717(16) . 12 ?
Cd1 Sb8 Ba4 69.73(2) 12 12 ?
Cd1 Sb8 Ba4 141.11(3) . 12 ?
Ba10 Sb8 Ba4 127.585(15) . 12 ?
Ba3 Sb8 Ba4 62.02(2) 12 12 ?
Ba3 Sb8 Ba4 139.45(3) . 12 ?
Ba11 Sb8 Ba4 76.47(2) . 12 ?
Ba4 Sb8 Ba4 104.82(3) . 12 ?
Cd3 Sb9 Ba8 75.19(3) . 7_545 ?
Cd3 Sb9 Ba8 75.19(3) . 14_456 ?
Ba8 Sb9 Ba8 76.30(3) 7_545 14_456 ?
Cd3 Sb9 Ba9 91.22(3) . . ?
Ba8 Sb9 Ba9 138.499(17) 7_545 . ?
Ba8 Sb9 Ba9 138.499(17) 14_456 . ?
Cd3 Sb9 Ba7 124.128(16) . 14_456 ?
Ba8 Sb9 Ba7 141.30(2) 7_545 14_456 ?
Ba8 Sb9 Ba7 77.52(2) 14_456 14_456 ?
Ba9 Sb9 Ba7 78.55(2) . 14_456 ?
Cd3 Sb9 Ba7 124.128(16) . 7_545 ?
Ba8 Sb9 Ba7 77.52(2) 7_545 7_545 ?
Ba8 Sb9 Ba7 141.30(2) 14_456 7_545 ?
Ba9 Sb9 Ba7 78.55(2) . 7_545 ?
Ba7 Sb9 Ba7 107.51(3) 14_456 7_545 ?
Cd3 Sb9 Ba10 144.85(3) . 2 ?
Ba8 Sb9 Ba10 77.343(17) 7_545 2 ?
Ba8 Sb9 Ba10 77.343(17) 14_456 2 ?
Ba9 Sb9 Ba10 123.93(3) . 2 ?
Ba7 Sb9 Ba10 69.432(15) 14_456 2 ?
Ba7 Sb9 Ba10 69.432(15) 7_545 2 ?
Cd3 Sb9 Ba6 59.949(17) . 14_456 ?
Ba8 Sb9 Ba6 128.07(2) 7_545 14_456 ?
Ba8 Sb9 Ba6 68.483(19) 14_456 14_456 ?
Ba9 Sb9 Ba6 70.770(17) . 14_456 ?
Ba7 Sb9 Ba6 64.88(2) 14_456 14_456 ?
Ba7 Sb9 Ba6 149.25(2) 7_545 14_456 ?
Ba10 Sb9 Ba6 127.247(15) 2 14_456 ?
Cd3 Sb9 Ba6 59.949(17) . 7_545 ?
Ba8 Sb9 Ba6 68.483(19) 7_545 7_545 ?
Ba8 Sb9 Ba6 128.07(2) 14_456 7_545 ?
Ba9 Sb9 Ba6 70.770(17) . 7_545 ?
Ba7 Sb9 Ba6 149.25(2) 14_456 7_545 ?
Ba7 Sb9 Ba6 64.88(2) 7_545 7_545 ?
Ba10 Sb9 Ba6 127.247(16) 2 7_545 ?
Ba6 Sb9 Ba6 105.49(3) 14_456 7_545 ?
Cd3 Sb10 Ba2 130.379(18) . . ?
Cd3 Sb10 Ba2 130.382(18) . 12 ?
Ba2 Sb10 Ba2 87.18(3) . 12 ?
Cd3 Sb10 Ba1 80.46(3) . . ?
Ba2 Sb10 Ba1 86.02(3) . . ?
Ba2 Sb10 Ba1 141.45(3) 12 . ?
Cd3 Sb10 Ba1 80.46(3) . 12 ?
Ba2 Sb10 Ba1 141.46(3) . 12 ?
Ba2 Sb10 Ba1 86.02(3) 12 12 ?
Ba1 Sb10 Ba1 76.27(3) . 12 ?
Cd3 Sb10 Ba9 87.53(3) . . ?
Ba2 Sb10 Ba9 72.81(2) . . ?
Ba2 Sb10 Ba9 72.81(2) 12 . ?
Ba1 Sb10 Ba9 139.556(16) . . ?
Ba1 Sb10 Ba9 139.557(16) 12 . ?
Cd3 Sb10 Ba6 61.820(17) . 7_545 ?
Ba2 Sb10 Ba6 68.63(2) . 7_545 ?
Ba2 Sb10 Ba6 139.89(2) 12 7_545 ?
Ba1 Sb10 Ba6 70.56(2) . 7_545 ?
Ba1 Sb10 Ba6 132.71(2) 12 7_545 ?
Ba9 Sb10 Ba6 69.726(17) . 7_545 ?
Cd3 Sb10 Ba6 61.820(17) . 14_456 ?
Ba2 Sb10 Ba6 139.89(2) . 14_456 ?
Ba2 Sb10 Ba6 68.64(2) 12 14_456 ?
Ba1 Sb10 Ba6 132.71(2) . 14_456 ?
Ba1 Sb10 Ba6 70.56(2) 12 14_456 ?
Ba9 Sb10 Ba6 69.726(17) . 14_456 ?
Ba6 Sb10 Ba6 109.93(3) 7_545 14_456 ?
Cd3 Sb10 Ba11 139.08(3) . . ?
Ba2 Sb10 Ba11 73.894(17) . . ?
Ba2 Sb10 Ba11 73.892(17) 12 . ?
Ba1 Sb10 Ba11 67.764(16) . . ?
Ba1 Sb10 Ba11 67.763(16) 12 . ?
Ba9 Sb10 Ba11 133.39(3) . . ?
Ba6 Sb10 Ba11 124.796(16) 7_545 . ?
Ba6 Sb10 Ba11 124.796(16) 14_456 . ?
Cd1 Sb11 Cd1 91.70(4) . 12 ?
Cd1 Sb11 Ba12 80.14(2) . . ?
Cd1 Sb11 Ba12 139.29(3) 12 . ?
Cd1 Sb11 Ba12 139.29(3) . 12 ?
Cd1 Sb11 Ba12 80.14(2) 12 12 ?
Ba12 Sb11 Ba12 80.72(3) . 12 ?
Cd1 Sb11 Ba11 64.29(2) . . ?
Cd1 Sb11 Ba11 64.29(2) 12 . ?
Ba12 Sb11 Ba11 139.388(15) . . ?
Ba12 Sb11 Ba11 139.388(15) 12 . ?
Cd1 Sb11 Ba5 142.02(3) . 12 ?
Cd1 Sb11 Ba5 65.94(2) 12 12 ?
Ba12 Sb11 Ba5 136.86(3) . 12 ?
Ba12 Sb11 Ba5 69.54(2) 12 12 ?
Ba11 Sb11 Ba5 78.127(19) . 12 ?
Cd1 Sb11 Ba5 65.94(2) . . ?
Cd1 Sb11 Ba5 142.02(3) 12 . ?
Ba12 Sb11 Ba5 69.54(2) . . ?
Ba12 Sb11 Ba5 136.86(3) 12 . ?
Ba11 Sb11 Ba5 78.127(19) . . ?
Ba5 Sb11 Ba5 112.89(3) 12 . ?
Cd1 Sb11 Ba10 66.62(2) . . ?
Cd1 Sb11 Ba10 66.62(2) 12 . ?
Ba12 Sb11 Ba10 73.63(2) . . ?
Ba12 Sb11 Ba10 73.63(2) 12 . ?
Ba11 Sb11 Ba10 106.74(3) . . ?
Ba5 Sb11 Ba10 123.403(15) 12 . ?
Ba5 Sb11 Ba10 123.404(15) . . ?
Sb6 Sb12 Ba5 119.034(16) 10_566 . ?
Sb6 Sb12 Ba5 119.035(16) 10_566 12 ?
Ba5 Sb12 Ba5 121.54(3) . 12 ?
Sb6 Sb12 Ba1 71.95(3) 10_566 12 ?
Ba5 Sb12 Ba1 135.84(3) . 12 ?
Ba5 Sb12 Ba1 70.30(2) 12 12 ?
Sb6 Sb12 Ba1 71.95(3) 10_566 . ?
Ba5 Sb12 Ba1 70.30(2) . . ?
Ba5 Sb12 Ba1 135.84(3) 12 . ?
Ba1 Sb12 Ba1 74.34(3) 12 . ?
Sb6 Sb12 Ba2 61.11(2) 10_566 10_566 ?
Ba5 Sb12 Ba2 70.45(2) . 10_566 ?
Ba5 Sb12 Ba2 137.38(2) 12 10_566 ?
Ba1 Sb12 Ba2 132.81(2) 12 10_566 ?
Ba1 Sb12 Ba2 86.47(2) . 10_566 ?
Sb6 Sb12 Ba2 61.110(19) 10_566 3 ?
Ba5 Sb12 Ba2 137.38(2) . 3 ?
Ba5 Sb12 Ba2 70.45(2) 12 3 ?
Ba1 Sb12 Ba2 86.47(2) 12 3 ?
Ba1 Sb12 Ba2 132.81(2) . 3 ?
Ba2 Sb12 Ba2 75.66(3) 10_566 3 ?
Sb6 Sb12 Ba11 127.08(3) 10_566 . ?
Ba5 Sb12 Ba11 75.559(15) . . ?
Ba5 Sb12 Ba11 75.558(15) 12 . ?
Ba1 Sb12 Ba11 66.494(18) 12 . ?
Ba1 Sb12 Ba11 66.493(18) . . ?
Ba2 Sb12 Ba11 142.165(15) 10_566 . ?
Ba2 Sb12 Ba11 142.165(15) 3 . ?
Ba2 Sb13 Ba2 91.09(3) 7_545 . ?
Ba2 Sb13 Ba1 142.791(17) 7_545 10_556 ?
Ba2 Sb13 Ba1 98.65(3) . 10_556 ?
Ba2 Sb13 Ba1 98.64(3) 7_545 16_545 ?
Ba2 Sb13 Ba1 142.789(16) . 16_545 ?
Ba1 Sb13 Ba1 94.96(3) 10_556 16_545 ?
Ba2 Sb13 Ba4 69.82(2) 7_545 7_545 ?
Ba2 Sb13 Ba4 73.27(2) . 7_545 ?
Ba1 Sb13 Ba4 147.339(14) 10_556 7_545 ?
Ba1 Sb13 Ba4 76.63(2) 16_545 7_545 ?
Ba2 Sb13 Ba4 73.27(2) 7_545 . ?
Ba2 Sb13 Ba4 69.82(2) . . ?
Ba1 Sb13 Ba4 76.63(2) 10_556 . ?
Ba1 Sb13 Ba4 147.338(14) 16_545 . ?
Ba4 Sb13 Ba4 126.29(3) 7_545 . ?
Ba2 Sb13 Ba5 75.483(19) 7_545 16_545 ?
Ba2 Sb13 Ba5 144.449(15) . 16_545 ?
Ba1 Sb13 Ba5 75.91(2) 10_556 16_545 ?
Ba1 Sb13 Ba5 72.56(2) 16_545 16_545 ?
Ba4 Sb13 Ba5 128.72(2) 7_545 16_545 ?
Ba4 Sb13 Ba5 74.78(2) . 16_545 ?
Ba2 Sb13 Ba5 144.448(15) 7_545 10_556 ?
Ba2 Sb13 Ba5 75.482(19) . 10_556 ?
Ba1 Sb13 Ba5 72.56(2) 10_556 10_556 ?
Ba1 Sb13 Ba5 75.91(2) 16_545 10_556 ?
Ba4 Sb13 Ba5 74.78(2) 7_545 10_556 ?
Ba4 Sb13 Ba5 128.72(2) . 10_556 ?
Ba5 Sb13 Ba5 132.61(3) 16_545 10_556 ?
Ba12 Sb14 Ba12 92.66(3) 16_545 13 ?
Ba12 Sb14 Ba8 90.60(2) 16_545 16_545 ?
Ba12 Sb14 Ba8 156.825(12) 13 16_545 ?
Ba12 Sb14 Ba8 156.825(12) 16_545 13 ?
Ba12 Sb14 Ba8 90.60(2) 13 13 ?
Ba8 Sb14 Ba8 95.36(3) 16_545 13 ?
Ba12 Sb14 Ba7 70.29(2) 16_545 4 ?
Ba12 Sb14 Ba7 73.22(2) 13 4 ?
Ba8 Sb14 Ba7 86.37(2) 16_545 4 ?
Ba8 Sb14 Ba7 132.348(18) 13 4 ?
Ba12 Sb14 Ba7 73.22(2) 16_545 . ?
Ba12 Sb14 Ba7 70.288(19) 13 . ?
Ba8 Sb14 Ba7 132.347(17) 16_545 . ?
Ba8 Sb14 Ba7 86.37(2) 13 . ?
Ba7 Sb14 Ba7 126.10(3) 4 . ?
Ba12 Sb14 Ba3 86.51(2) 16_545 . ?
Ba12 Sb14 Ba3 133.713(18) 13 . ?
Ba8 Sb14 Ba3 69.38(2) 16_545 . ?
Ba8 Sb14 Ba3 74.80(2) 13 . ?
Ba7 Sb14 Ba3 146.370(10) 4 . ?
Ba7 Sb14 Ba3 65.225(17) . . ?
Ba12 Sb14 Ba3 133.714(19) 16_545 4 ?
Ba12 Sb14 Ba3 86.51(2) 13 4 ?
Ba8 Sb14 Ba3 74.80(2) 16_545 4 ?
Ba8 Sb14 Ba3 69.38(2) 13 4 ?
Ba7 Sb14 Ba3 65.228(17) 4 4 ?
Ba7 Sb14 Ba3 146.371(10) . 4 ?
Ba3 Sb14 Ba3 125.71(3) . 4 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ba1 Sb13 3.4356(9) 10_566 ?
Ba1 Sb4 3.5458(12) 7_545 ?
Ba1 Sb10 3.6115(10) . ?
Ba1 Sb12 3.6913(10) . ?
Ba1 Sb6 3.9191(12) 10_566 ?
Ba1 Sb2 3.9378(10) . ?
Ba1 Ba5 4.1678(13) . ?
Ba1 Ba11 4.2284(10) . ?
Ba1 Ba4 4.3268(13) 10_566 ?
Ba1 Ba5 4.3318(12) 7_545 ?
Ba1 Ba6 4.3424(11) 7_545 ?
Ba1 Ba1 4.4603(16) 12 ?
Ba2 Sb13 3.4279(9) . ?
Ba2 Sb10 3.4728(10) . ?
Ba2 Sb6 3.5622(9) . ?
Ba2 Sb3 3.8318(12) 7_545 ?
Ba2 Sb12 3.9043(11) 10_556 ?
Ba2 Ba4 3.9898(13) . ?
Ba2 Sb2 4.0337(11) 7_545 ?
Ba2 Sb2 4.0488(11) . ?
Ba2 Ba4 4.1600(12) 7_545 ?
Ba2 Ba6 4.1692(11) 7_545 ?
Ba2 Ba5 4.3066(13) 10_556 ?
Ba2 Ba9 4.3510(12) . ?
Ba3 Sb5 3.3653(10) . ?
Ba3 Sb3 3.4472(11) . ?
Ba3 Sb4 3.5233(10) 16_545 ?
Ba3 Sb8 3.5891(10) . ?
Ba3 Sb1 3.6486(12) . ?
Ba3 Sb14 3.6943(9) . ?
Ba3 Ba4 3.7506(13) . ?
Ba3 Ba7 3.9756(11) . ?
Ba3 Cd1 3.9941(12) . ?
Ba3 Ba8 4.0474(13) 16_545 ?
Ba3 Cd2 4.0901(11) . ?
Ba3 Ba8 4.3176(14) 13 ?
Ba4 Sb2 3.4442(12) . ?
Ba4 Sb6 3.4554(10) . ?
Ba4 Sb4 3.5106(11) 16_545 ?
Ba4 Sb3 3.5152(10) . ?
Ba4 Sb13 3.5418(9) . ?
Ba4 Cd2 3.5603(10) . ?
Ba4 Sb8 3.6895(10) . ?
Ba4 Cd1 3.8735(11) . ?
Ba4 Ba2 4.1601(12) 7_545 ?
Ba4 Ba1 4.3268(13) 10_556 ?
Ba5 Sb3 3.3938(10) 16 ?
Ba5 Sb2 3.4664(11) . ?
Ba5 Sb12 3.5447(10) . ?
Ba5 Sb13 3.6042(9) 10_566 ?
Ba5 Cd1 3.6953(11) . ?
Ba5 Sb11 3.7119(10) . ?
Ba5 Sb4 3.8271(12) . ?
Ba5 Ba12 4.1314(13) . ?
Ba5 Ba2 4.3066(13) 10_566 ?
Ba5 Ba1 4.3319(12) 7_545 ?
Ba5 Ba4 4.3398(11) 16 ?
Ba6 Sb3 3.3783(12) . ?
Ba6 Sb4 3.4150(12) . ?
Ba6 Sb2 3.5341(10) . ?
Ba6 Sb1 3.5684(10) . ?
Ba6 Cd3 3.6026(11) 14_556 ?
Ba6 Cd1 3.7656(14) . ?
Ba6 Sb10 3.8964(11) 14_556 ?
Ba6 Sb9 4.0082(11) 14_556 ?
Ba6 Ba7 4.1274(12) . ?
Ba6 Ba2 4.1693(11) 7_545 ?
Ba6 Ba8 4.2569(11) . ?
Ba6 Ba1 4.3424(11) 7_545 ?
Ba7 Sb7 3.4812(10) 14_556 ?
Ba7 Sb1 3.5188(10) . ?
Ba7 Sb1 3.5790(11) 13 ?
Ba7 Sb3 3.6404(11) . ?
Ba7 Sb9 3.6672(10) 14_556 ?
Ba7 Sb14 3.6822(10) . ?
Ba7 Ba12 4.0787(11) 13 ?
Ba7 Ba12 4.2250(13) 16_545 ?
Ba7 Ba10 4.3363(11) 13 ?
Ba7 Ba8 4.5035(15) . ?
Ba8 Sb14 3.4045(9) 13 ?
Ba8 Sb4 3.5018(12) . ?
Ba8 Sb9 3.5237(10) 14_556 ?
Ba8 Sb5 3.5697(10) 13 ?
Ba8 Sb5 3.6598(11) 5 ?
Ba8 Cd3 3.9900(12) 14_556 ?
Ba8 Ba3 4.0474(13) 16 ?
Ba8 Ba3 4.3177(14) 13 ?
Ba8 Ba8 4.3536(16) 12_655 ?
Ba8 Ba10 4.6728(11) 13 ?
Ba9 Sb3 3.3301(11) 14_456 ?
Ba9 Sb3 3.3301(11) 7_545 ?
Ba9 Sb9 3.6099(13) . ?
Ba9 Sb10 3.8414(13) . ?
Ba9 Sb7 3.9998(15) . ?
Ba9 Ba2 4.3511(12) 12 ?
Ba9 Ba12 4.3692(11) 3_545 ?
Ba9 Ba12 4.3692(11) 10_556 ?
Ba9 Ba6 4.4233(12) 7_545 ?
Ba9 Ba6 4.4233(12) 14_456 ?
Ba9 Ba7 4.6070(11) 7_545 ?
Ba10 Sb1 3.5819(12) . ?
Ba10 Sb1 3.5820(12) 12 ?
Ba10 Sb8 3.5823(13) . ?
Ba10 Cd1 3.8057(11) 12 ?
Ba10 Cd1 3.8058(11) . ?
Ba10 Sb11 3.8257(13) . ?
Ba10 Sb9 3.9367(15) 2_554 ?
Ba10 Sb7 3.9798(13) 2_554 ?
Ba10 Sb5 4.0414(16) . ?
Ba10 Ba7 4.3362(10) 8_455 ?
Ba10 Ba7 4.3362(10) 13 ?
Ba11 Cd1 3.5757(11) . ?
Ba11 Cd1 3.5758(11) 12 ?
Ba11 Sb2 3.5785(12) . ?
Ba11 Sb2 3.5786(12) 12 ?
Ba11 Sb8 3.5975(12) . ?
Ba11 Sb11 3.6512(12) . ?
Ba11 Sb10 3.9558(15) . ?
Ba11 Sb12 4.0063(16) . ?
Ba11 Sb6 4.0423(15) . ?
Ba11 Ba1 4.2283(10) 12 ?
Ba11 Ba2 4.4818(11) 12 ?
Ba12 Sb14 3.3914(9) 13 ?
Ba12 Sb11 3.5281(9) . ?
Ba12 Sb1 3.6006(12) . ?
Ba12 Sb3 3.6207(10) 16 ?
Ba12 Sb7 3.6368(10) 10_566 ?
Ba12 Sb7 3.6679(11) 2_554 ?
Ba12 Ba7 4.0786(11) 13 ?
Ba12 Ba7 4.2251(13) 16 ?
Ba12 Ba9 4.3693(11) 10_566 ?
Ba12 Ba12 4.5694(16) 12 ?
Cd1 Sb1 2.9182(10) . ?
Cd1 Sb11 2.9854(10) . ?
Cd1 Sb8 3.0180(10) . ?
Cd1 Sb2 3.0902(10) . ?
Cd2 Sb4 2.8756(9) 5_445 ?
Cd2 Sb4 2.8756(9) 16_545 ?
Cd2 Sb8 2.9498(14) . ?
Cd2 Sb6 3.0245(13) . ?
Cd2 Cd3 3.0989(14) 10_556 ?
Cd2 Ba4 3.5603(10) 12 ?
Cd2 Ba3 4.0900(11) 12 ?
Cd3 Sb10 2.9275(12) . ?
Cd3 Sb9 2.9778(12) . ?
Cd3 Sb4 2.9842(10) 7_545 ?
Cd3 Sb4 2.9842(10) 14_456 ?
Cd3 Cd2 3.0990(14) 10_566 ?
Cd3 Ba6 3.6026(11) 14_456 ?
Cd3 Ba6 3.6026(11) 7_545 ?
Cd3 Ba8 3.9900(12) 7_545 ?
Cd3 Ba8 3.9900(12) 14_456 ?
Sb1 Ba7 3.5789(11) 13 ?
Sb2 Ba2 4.0339(11) 7_545 ?
Sb3 Ba9 3.3301(11) 14_556 ?
Sb3 Ba5 3.3939(10) 16_545 ?
Sb3 Ba12 3.6208(10) 16_545 ?
Sb3 Ba2 3.8320(12) 7_545 ?
Sb4 Cd2 2.8757(9) 5 ?
Sb4 Cd3 2.9842(10) 14_556 ?
Sb4 Ba4 3.5107(11) 16 ?
Sb4 Ba3 3.5232(10) 16 ?
Sb4 Ba1 3.5459(12) 7_545 ?
Sb5 Sb5 2.8236(15) 9 ?
Sb5 Ba3 3.3653(10) 12 ?
Sb5 Ba8 3.5696(10) 8_455 ?
Sb5 Ba8 3.5696(10) 13 ?
Sb5 Ba8 3.6598(11) 5_445 ?
Sb5 Ba8 3.6598(11) 16_545 ?
Sb6 Sb12 2.8879(12) 10_556 ?
Sb6 Ba4 3.4554(10) 12 ?
Sb6 Ba2 3.5621(10) 12 ?
Sb6 Ba1 3.9190(12) 3_545 ?
Sb6 Ba1 3.9190(12) 10_556 ?
Sb7 Sb7 2.8999(16) 9_556 ?
Sb7 Ba7 3.4811(10) 7_545 ?
Sb7 Ba7 3.4811(10) 14_456 ?
Sb7 Ba12 3.6368(10) 3_545 ?
Sb7 Ba12 3.6368(10) 10_556 ?
Sb7 Ba12 3.6678(11) 11_566 ?
Sb7 Ba12 3.6678(11) 2 ?
Sb7 Ba10 3.9798(13) 2 ?
Sb8 Cd1 3.0180(10) 12 ?
Sb8 Ba3 3.5891(10) 12 ?
Sb8 Ba4 3.6896(10) 12 ?
Sb9 Ba8 3.5237(10) 7_545 ?
Sb9 Ba8 3.5237(10) 14_456 ?
Sb9 Ba7 3.6673(10) 14_456 ?
Sb9 Ba7 3.6673(10) 7_545 ?
Sb9 Ba10 3.9367(15) 2 ?
Sb9 Ba6 4.0081(11) 14_456 ?
Sb9 Ba6 4.0081(11) 7_545 ?
Sb10 Ba2 3.4729(10) 12 ?
Sb10 Ba1 3.6116(10) 12 ?
Sb10 Ba6 3.8964(11) 7_545 ?
Sb10 Ba6 3.8964(11) 14_456 ?
Sb11 Cd1 2.9854(10) 12 ?
Sb11 Ba12 3.5282(9) 12 ?
Sb11 Ba5 3.7119(10) 12 ?
Sb12 Sb6 2.8879(12) 10_566 ?
Sb12 Ba5 3.5448(10) 12 ?
Sb12 Ba1 3.6912(10) 12 ?
Sb12 Ba2 3.9042(11) 10_566 ?
Sb12 Ba2 3.9042(11) 3 ?
Sb13 Ba2 3.4279(9) 7_545 ?
Sb13 Ba1 3.4357(9) 10_556 ?
Sb13 Ba1 3.4357(9) 16_545 ?
Sb13 Ba4 3.5418(9) 7_545 ?
Sb13 Ba5 3.6042(9) 16_545 ?
Sb13 Ba5 3.6042(9) 10_556 ?
Sb14 Ba12 3.3913(9) 16_545 ?
Sb14 Ba12 3.3913(9) 13 ?
Sb14 Ba8 3.4045(9) 16_545 ?
Sb14 Ba8 3.4045(9) 13 ?
Sb14 Ba7 3.6821(10) 4 ?
Sb14 Ba3 3.6944(9) 4 ?
